# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1940343'
loop_
_audit_author_name
_audit_author_address
'Jun-Wei Zhao'
;Henan University
China
;
_audit_update_record             
;
2019-09-07 deposited with the CCDC.	2019-09-23 downloaded from the CCDC.
;

# start Validation Reply Form

_vrf_PLAT975_1                   
;
PROBLEM:  Check Calcd Resid. Dens.  1.05A   From O8W             2.14 eA-3
RESPONSE: Due to the large structure and the existence of a large 
 amount of weight atoms, the intensity data are not very good, 
leading to the ADP max/min ratio of some water molecules, and it is 
very difficult to refine this large structure, therefore, 
 in the final refinement, the MO, Ge, Cu and La atoms were refined 
anisotropically, some O atoms and water molecules were
 refined isotropically. Thus, the isotropical refinement and the isotropic 
atomic displacement parameter restriction of O8W leads to
 the occurrence of a residual density near to O8W.
;

_vrf_PLAT201_1                   
;
PROBLEM: Isotropic non-H Atoms in Main Residue(s) .......    2 Report 
RESPONSE: Due to the large structure and the existence of a large 
 amount of weight atoms, the intensity data are not very good, 
 leading to the ADP max/min ratio of some water molecules, and it is 
very difficult to refine this large structure, therefore, 
 in the final refinement, the MO, Ge, Cu and La atoms were refined 
anisotropically, some O atoms and water molecules were
 refined isotropically.
;

_vrf_PLAT306_1                   
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) ....... O9W Check
RESPONSE: The hydrogen atoms of the water molecules could not be directly 
 located from the difference Fourier maps because of the presence of too many
 heavy atoms in the structure.
;

_vrf_PLAT430_1                   
;
PROBLEM: Short Inter D...A Contact O1W ..O9W . 2.80 Ang.
RESPONSE: In the crystal structure, there are a number of short contacts between 
Ow(H2O) and O(POM) or Ow(H2O) in the range of 2.61-2.89 Ang, which indicate 
extensive hydrogen bonding interactions among them. 
;

# end Validation Reply Form



_audit_creation_date             2019-09-07
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        
;
 ? 
;
_chemical_formula_moiety         
'C60 H40 Cu5 Ge2 La2 Mo24 N10 O114, 2(N), 12(O)'
_chemical_formula_sum            'C60 H124 Cu5 Ge2 La2 Mo24 N12 O139'
_chemical_formula_weight         6280.96
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        P2(1)/c
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   19.4250(4)
_cell_length_b                   14.3964(3)
_cell_length_c                   28.9317(6)
_cell_angle_alpha                90
_cell_angle_beta                 101.4280(10)
_cell_angle_gamma                90
_cell_volume                     7930.3(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9050
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      28.09
_cell_measurement_theta_min      2.56
_shelx_estimated_absorpt_T_max   0.349
_shelx_estimated_absorpt_T_min   0.273
_exptl_absorpt_coefficient_mu    3.505
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.5916
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. 
wR2(int) was 0.1437 before and 0.0723 after correction. The Ratio 
of minimum to maximum transmission is 0.7933. 
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            green
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    2.630
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             6022
_exptl_crystal_size_max          0.5
_exptl_crystal_size_mid          0.47
_exptl_crystal_size_min          0.38
_exptl_special_details           
;
 ? 
;
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0560
_diffrn_reflns_av_unetI/netI     0.0483
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            60571
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_min         2.145
_diffrn_ambient_temperature      150.02
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    ?
_reflns_Friedel_fraction_max     ?
_reflns_number_gt                11129
_reflns_number_total             13899
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_refine_diff_density_max         2.142
_refine_diff_density_min         -1.554
_refine_diff_density_rms         0.170
_refine_ls_extinction_coef       0.00014(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1059
_refine_ls_number_reflns         13899
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.0639
_refine_ls_R_factor_gt           0.0477
_refine_ls_restrained_S_all      1.042
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0455P)²+58.9580P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1086
_refine_ls_wR_factor_ref         0.1166
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(O6W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
3. Others
 Fixed Sof: La1(0.85) La1B(0.15) Mo1(0.75) Mo1B(0.25) Mo2(0.75) Mo2B(0.25)
 Mo3(0.75) Mo3B(0.25) Mo4(0.75) Mo4B(0.25) Mo6(0.75) Mo6B(0.25) Mo9(0.75)
 Mo9B(0.25)
 Fixed Uiso: O7W(0.05741) O8W(0.06)
4.a Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C3(H3), C4(H4), C7(H7), C8(H8), C9(H9), C10(H10), C13(H13),
 C14(H14), C15(H15), C16(H16), C19(H19), C20(H20), C21(H21), C22(H22), C25(H25),
  C26(H26), C27(H27), C28(H28)
;
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La 0.20907(3) 0.34568(5) 0.46654(2) 0.02027(13) Uani 0.85 1 d . . . . .
La1B La 0.21496(14) 0.2957(2) 0.47444(9) 0.0114(6) Uiso 0.15 1 d . . . . .
Ge1 Ge 0.25665(4) 0.00756(5) 0.26592(2) 0.01580(17) Uani 1 1 d . . . . .
Mo1 Mo 0.43735(5) -0.04051(9) 0.27625(3) 0.0266(2) Uani 0.75 1 d . . . . .
Mo1B Mo 0.42835(15) -0.0839(2) 0.27094(10) 0.0152(7) Uiso 0.25 1 d . . . . .
Mo2 Mo 0.07839(5) 0.05760(9) 0.26851(3) 0.0199(2) Uani 0.75 1 d . . . . .
Mo2B Mo 0.08655(15) 0.0964(2) 0.26141(10) 0.0104(7) Uiso 0.25 1 d . . . . .
Mo3 Mo 0.38996(5) 0.08854(7) 0.36023(4) 0.0248(2) Uani 0.75 1 d . . . . .
Mo3B Mo 0.40320(16) 0.0912(2) 0.34267(10) 0.0138(8) Uiso 0.25 1 d . . . . .
Mo4 Mo 0.17116(5) 0.16436(7) 0.18046(4) 0.0207(2) Uani 0.75 1 d . . . . .
Mo4B Mo 0.18099(14) 0.14396(19) 0.16317(10) 0.0104(7) Uiso 0.25 1 d . . . . .
Mo5 Mo 0.35047(4) -0.13554(5) 0.35555(2) 0.02973(18) Uani 1 1 d . . . . .
Mo6 Mo 0.17153(6) -0.05883(6) 0.35975(4) 0.0217(2) Uani 0.75 1 d . . . . .
Mo6B Mo 0.14999(15) -0.0666(2) 0.34172(10) 0.0125(7) Uiso 0.25 1 d . . . . .
Mo7 Mo 0.33746(4) 0.09300(5) 0.17572(2) 0.02957(18) Uani 1 1 d . . . . .
Mo8 Mo 0.20272(4) -0.22789(5) 0.26468(2) 0.02902(17) Uani 1 1 d . . . . .
Mo9 Mo 0.29861(5) -0.16304(7) 0.18936(4) 0.0224(2) Uani 0.75 1 d . . . . .
Mo9B Mo 0.28186(15) -0.1471(2) 0.17044(10) 0.0151(8) Uiso 0.25 1 d . . . . .
Mo10 Mo 0.12830(4) -0.09131(5) 0.17602(2) 0.02659(17) Uani 1 1 d . . . . .
Mo11 Mo 0.30657(4) 0.24199(5) 0.25681(2) 0.02537(17) Uani 1 1 d . . . . .
Mo12 Mo 0.20671(4) 0.16256(5) 0.34724(2) 0.02585(17) Uani 1 1 d . . . . .
Cu1 Cu -0.08331(5) 0.26950(7) 0.49214(3) 0.0262(2) Uani 1 1 d . . . . .
Cu2 Cu 0.500000 0.500000 0.500000 0.0245(3) Uani 1 2 d S T P . .
Cu3 Cu 0.25344(5) 0.50355(7) 0.27721(4) 0.0343(3) Uani 1 1 d . . . . .
N1 N -0.0791(3) 0.3247(4) 0.5547(2) 0.0239(14) Uani 1 1 d . . . . .
N2 N -0.0844(3) 0.2051(4) 0.4320(2) 0.0241(14) Uani 1 1 d . . . . .
N3 N 0.4916(3) 0.4497(4) 0.4354(2) 0.0244(14) Uani 1 1 d . . . . .
N4 N 0.3434(4) 0.5691(4) 0.2836(3) 0.0362(18) Uani 1 1 d . . . . .
N5 N 0.1641(3) 0.4369(5) 0.2697(2) 0.0323(16) Uani 1 1 d . . . . .
N6 N 0.3580(5) 0.7661(6) 0.0351(3) 0.060(2) Uani 1 1 d . . . . .
O1W O -0.0342(4) 0.1161(5) 0.5396(3) 0.061(2) Uani 1 1 d . . . . .
O2W O -0.1353(4) 0.4105(4) 0.45360(19) 0.0492(18) Uani 1 1 d . . . . .
O3W O 0.4495(4) 0.6493(5) 0.4731(3) 0.067(2) Uani 1 1 d . . . . .
O4W O 0.2449(4) 0.5142(5) 0.4845(3) 0.0561(18) Uani 1 1 d . . . . .
O5W O 0.3024(3) 0.3663(5) 0.5413(2) 0.0500(18) Uani 1 1 d . . . . .
O6W O 0.1059(4) 0.4465(6) 0.4814(4) 0.090(3) Uani 1 1 d . U . . .
O7W O 0.1738(4) 0.3048(5) 0.5449(2) 0.057 Uiso 1 1 d . . . . .
O8W O 0.2608(4) 0.1872(5) 0.4855(2) 0.060 Uiso 1 1 d . . . . .
O9W O 1.1120(5) 1.3638(7) 0.0554(3) 0.096(3) Uani 1 1 d . . . . .
O10W O -0.2500(8) 0.0645(9) 0.4775(5) 0.165(6) Uani 1 1 d . . . . .
O11W O 0.7225(4) 0.4057(6) 0.4332(3) 0.073(2) Uani 1 1 d . . . . .
O12W O 0.6850(3) 1.0950(4) 0.0776(2) 0.0461(16) Uani 1 1 d . . . . .
O13W O 1.2297(6) 1.3874(7) 0.1286(3) 0.104(3) Uani 1 1 d . . . . .
O1 O 0.5137(3) -0.0818(6) 0.2642(2) 0.059(2) Uani 1 1 d . . . . .
O2 O 0.3367(2) -0.0156(3) 0.30301(17) 0.0194(11) Uani 1 1 d . . . . .
O3 O 0.3573(2) 0.2131(3) 0.20940(16) 0.0198(11) Uani 1 1 d . . . . .
O4 O 0.2658(2) 0.0992(3) 0.22915(15) 0.0184(10) Uani 1 1 d . . . . .
O5 O 0.2526(3) 0.1432(4) 0.14215(16) 0.0251(12) Uani 1 1 d . . . . .
O6 O 0.1952(2) 0.0361(3) 0.29967(15) 0.0164(10) Uani 1 1 d . . . . .
O7 O 0.0779(3) -0.0150(4) 0.31767(18) 0.0262(12) Uani 1 1 d . . . . .
O8 O 0.3078(2) -0.0314(3) 0.16342(16) 0.0214(11) Uani 1 1 d . . . . .
O9 O 0.3695(3) 0.1784(3) 0.30340(17) 0.0241(12) Uani 1 1 d . . . . .
O10 O 0.1629(3) -0.1577(3) 0.30665(17) 0.0230(11) Uani 1 1 d . . . . .
O11 O 0.2390(2) 0.2257(3) 0.29960(15) 0.0183(10) Uani 1 1 d . . . . .
O12 O 0.1132(3) 0.1637(3) 0.31408(16) 0.0211(11) Uani 1 1 d . . . . .
O13 O 0.4050(3) 0.0395(4) 0.22857(17) 0.0256(12) Uani 1 1 d . . . . .
O14 O 0.2056(3) 0.2457(4) 0.38894(16) 0.0255(12) Uani 1 1 d . . . . .
O15 O 0.1874(3) -0.3387(4) 0.27905(18) 0.0290(12) Uani 1 1 d . . . . .
O16 O 0.2284(2) -0.0894(3) 0.23232(17) 0.0204(11) Uani 1 1 d . . . . .
O17 O 0.3727(3) -0.1352(4) 0.23260(19) 0.0288(12) Uani 1 1 d . . . . .
O18 O 0.3033(3) 0.1190(3) 0.36718(16) 0.0237(11) Uani 1 1 d . . . . .
O19 O 0.1275(3) -0.2052(3) 0.21383(17) 0.0218(11) Uani 1 1 d . . . . .
O20 O 0.1797(3) 0.0572(3) 0.38440(16) 0.0217(11) Uani 1 1 d . . . . .
O21 O 0.1202(2) 0.1442(3) 0.22260(17) 0.0223(11) Uani 1 1 d . . . . .
O22 O 0.1517(2) 0.0304(3) 0.16036(16) 0.0208(11) Uani 1 1 d . . . . .
O23 O 0.2630(3) -0.0889(3) 0.37111(17) 0.0224(11) Uani 1 1 d . . . . .
O24 O 0.1170(3) 0.2149(4) 0.1331(2) 0.0443(17) Uani 1 1 d . . . . .
O25 O 0.1329(3) -0.1177(4) 0.3973(2) 0.0418(16) Uani 1 1 d . . . . .
O26 O 0.0866(2) -0.0296(3) 0.22427(16) 0.0190(11) Uani 1 1 d . . . . .
O27 O 0.2234(2) 0.2632(3) 0.20690(17) 0.0220(11) Uani 1 1 d . . . . .
O28 O 0.4632(3) 0.0394(4) 0.3234(2) 0.0347(14) Uani 1 1 d . . . . .
O29 O 0.2618(3) -0.2565(3) 0.21801(18) 0.0253(12) Uani 1 1 d . . . . .
O30 O 0.3759(3) -0.2138(4) 0.39882(18) 0.0347(14) Uani 1 1 d . . . . .
O31 O 0.2926(2) -0.2049(3) 0.30893(17) 0.0214(11) Uani 1 1 d . . . . .
O32 O 0.4287(3) -0.1401(4) 0.32528(18) 0.0272(12) Uani 1 1 d . . . . .
O33 O 0.0569(3) -0.1107(4) 0.13374(17) 0.0277(12) Uani 1 1 d . . . . .
O34 O 0.3897(3) 0.1094(4) 0.13647(17) 0.0284(12) Uani 1 1 d . . . . .
O35 O -0.0045(3) 0.0968(5) 0.25227(19) 0.0447(17) Uani 1 1 d . . . . .
O36 O 0.4461(3) 0.1543(4) 0.3966(2) 0.0506(18) Uani 1 1 d . . . . .
O37 O 0.3955(3) -0.0243(4) 0.38917(17) 0.0259(12) Uani 1 1 d . . . . .
O38 O 0.1976(3) -0.1457(4) 0.14767(17) 0.0263(12) Uani 1 1 d . . . . .
O39 O 0.3281(3) 0.3546(3) 0.26871(18) 0.0262(12) Uani 1 1 d . . . . .
O40 O 0.3306(3) -0.2194(4) 0.1458(2) 0.0487(18) Uani 1 1 d . . . . .
O41 O -0.2530(3) 0.2484(4) 0.54687(19) 0.0320(13) Uani 1 1 d . . . . .
O42 O -0.1776(3) 0.2322(4) 0.49892(18) 0.0318(13) Uani 1 1 d . . . . .
O43 O 0.0136(3) 0.3020(4) 0.48543(19) 0.0338(14) Uani 1 1 d . . . . .
O44 O 0.0928(3) 0.2664(5) 0.4429(2) 0.0499(19) Uani 1 1 d . . . . .
O45 O 0.4061(3) 0.4427(4) 0.49481(16) 0.0253(12) Uani 1 1 d . . . . .
O46 O 0.3241(3) 0.3654(4) 0.44370(18) 0.0297(13) Uani 1 1 d . . . . .
O47 O 0.3170(4) 0.5524(6) 0.1597(3) 0.069(2) Uani 1 1 d . . . . .
O48 O 0.2514(3) 0.5086(5) 0.2111(2) 0.0459(16) Uani 1 1 d . . . . .
O49 O 0.2504(3) 0.4933(4) 0.3450(2) 0.0361(14) Uani 1 1 d . . . . .
O50 O 0.1833(3) 0.4386(4) 0.3934(2) 0.0428(15) Uani 1 1 d . . . . .
C1 C -0.0254(4) 0.3673(6) 0.5826(3) 0.0314(19) Uani 1 1 d . . . . .
H1 H 0.015960 0.379493 0.570813 0.038 Uiso 1 1 calc R . . . .
C2 C -0.0278(4) 0.3944(5) 0.6282(3) 0.0275(18) Uani 1 1 d . . . . .
H2 H 0.010753 0.426028 0.646920 0.033 Uiso 1 1 calc R . . . .
C3 C -0.0879(4) 0.3746(5) 0.6461(2) 0.0239(17) Uani 1 1 d . . . . .
H3 H -0.090251 0.390276 0.677677 0.029 Uiso 1 1 calc R . . . .
C4 C -0.1433(4) 0.3320(5) 0.6171(3) 0.0274(18) Uani 1 1 d . . . . .
H4 H -0.185113 0.318578 0.628195 0.033 Uiso 1 1 calc R . . . .
C5 C -0.1376(4) 0.3085(5) 0.5712(3) 0.0214(16) Uani 1 1 d . . . . .
C6 C -0.1944(4) 0.2599(6) 0.5380(3) 0.0264(17) Uani 1 1 d . . . . .
C7 C -0.1379(4) 0.1620(6) 0.4042(3) 0.036(2) Uani 1 1 d . . . . .
H7 H -0.182512 0.161650 0.412978 0.043 Uiso 1 1 calc R . . . .
C8 C -0.1304(4) 0.1181(7) 0.3634(3) 0.038(2) Uani 1 1 d . . . . .
H8 H -0.169737 0.089175 0.343955 0.045 Uiso 1 1 calc R . . . .
C9 C -0.0665(5) 0.1161(7) 0.3510(3) 0.039(2) Uani 1 1 d . . . . .
H9 H -0.060333 0.084646 0.323246 0.047 Uiso 1 1 calc R . . . .
C10 C -0.0105(5) 0.1609(6) 0.3795(3) 0.034(2) Uani 1 1 d . . . . .
H10 H 0.034601 0.161449 0.371421 0.040 Uiso 1 1 calc R . . . .
C11 C -0.0218(4) 0.2043(5) 0.4195(3) 0.0249(17) Uani 1 1 d . . . . .
C12 C 0.0333(4) 0.2606(6) 0.4514(3) 0.0313(19) Uani 1 1 d . . . . .
C13 C 0.5390(4) 0.4531(6) 0.4078(3) 0.0296(19) Uani 1 1 d . . . . .
H13 H 0.582542 0.483751 0.418684 0.036 Uiso 1 1 calc R . . . .
C14 C 0.5256(4) 0.4125(6) 0.3633(3) 0.034(2) Uani 1 1 d . . . . .
H14 H 0.559793 0.415097 0.343931 0.040 Uiso 1 1 calc R . . . .
C15 C 0.4622(4) 0.3683(6) 0.3475(3) 0.0302(19) Uani 1 1 d . . . . .
H15 H 0.452459 0.340062 0.317213 0.036 Uiso 1 1 calc R . . . .
C16 C 0.4135(4) 0.3657(5) 0.3759(3) 0.0246(17) Uani 1 1 d . . . . .
H16 H 0.369130 0.337097 0.365334 0.030 Uiso 1 1 calc R . . . .
C17 C 0.4302(4) 0.4056(5) 0.4206(3) 0.0207(16) Uani 1 1 d . . . . .
C18 C 0.3827(4) 0.4044(5) 0.4553(3) 0.0237(17) Uani 1 1 d . . . . .
C19 C 0.3864(5) 0.5992(6) 0.3227(4) 0.046(2) Uani 1 1 d . . . . .
H19 H 0.375043 0.587975 0.352628 0.055 Uiso 1 1 calc R . . . .
C20 C 0.4487(5) 0.6477(6) 0.3197(4) 0.050(3) Uani 1 1 d . . . . .
H20 H 0.479122 0.669040 0.347521 0.061 Uiso 1 1 calc R . . . .
C21 C 0.4650(5) 0.6638(7) 0.2761(5) 0.056(3) Uani 1 1 d . . . . .
H21 H 0.506628 0.696415 0.273530 0.067 Uiso 1 1 calc R . . . .
C22 C 0.4210(5) 0.6325(7) 0.2369(4) 0.054(3) Uani 1 1 d . . . . .
H22 H 0.431168 0.643211 0.206564 0.065 Uiso 1 1 calc R . . . .
C23 C 0.3606(4) 0.5844(6) 0.2416(3) 0.038(2) Uani 1 1 d . . . . .
C24 C 0.3084(5) 0.5477(7) 0.2009(4) 0.049(3) Uani 1 1 d . . . . .
C25 C 0.1228(4) 0.4095(6) 0.2296(3) 0.033(2) Uani 1 1 d . . . . .
H25 H 0.136185 0.422983 0.200451 0.040 Uiso 1 1 calc R . . . .
C26 C 0.0609(5) 0.3619(6) 0.2293(4) 0.041(2) Uani 1 1 d . . . . .
H26 H 0.032505 0.342099 0.200426 0.049 Uiso 1 1 calc R . . . .
C27 C 0.0412(5) 0.3436(6) 0.2712(3) 0.038(2) Uani 1 1 d . . . . .
H27 H -0.001220 0.311084 0.271666 0.045 Uiso 1 1 calc R . . . .
C28 C 0.0830(4) 0.3726(6) 0.3127(3) 0.036(2) Uani 1 1 d . . . . .
H28 H 0.069871 0.361212 0.342138 0.043 Uiso 1 1 calc R . . . .
C29 C 0.1442(4) 0.4185(5) 0.3105(3) 0.032(2) Uani 1 1 d . . . . .
C30 C 0.1951(5) 0.4516(6) 0.3529(3) 0.036(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1B 0.757(3) . ?
La1 O4W 2.549(7) . ?
La1 O5W 2.549(5) . ?
La1 O6W 2.579(8) . ?
La1 O7W 2.564(7) . ?
La1 O8W 2.509(8) . ?
La1 O14 2.656(5) . ?
La1 O44 2.502(5) . ?
La1 O46 2.469(5) . ?
La1 O50 2.468(6) . ?
La1B O5W 2.522(6) . ?
La1B O7W 2.337(7) . ?
La1B O8W 1.795(8) . ?
La1B O14 2.548(5) . ?
La1B O44 2.404(6) . ?
La1B O46 2.654(6) . ?
Ge1 O2 1.737(5) . ?
Ge1 O4 1.726(5) . ?
Ge1 O6 1.734(4) . ?
Ge1 O16 1.727(5) . ?
Mo1 Mo1B 0.658(3) . ?
Mo1 Mo3B 2.869(3) . ?
Mo1 O1 1.697(6) . ?
Mo1 O2 2.270(5) . ?
Mo1 O13 1.812(5) . ?
Mo1 O17 2.099(6) . ?
Mo1 O28 1.780(6) . ?
Mo1 O32 2.047(5) . ?
Mo1B Mo5 3.209(3) . ?
Mo1B O1 1.708(7) . ?
Mo1B O2 2.378(5) . ?
Mo1B O13 2.155(6) . ?
Mo1B O17 1.572(6) . ?
Mo1B O28 2.347(7) . ?
Mo1B O32 1.767(6) . ?
Mo2 Mo2B 0.627(2) . ?
Mo2 Mo6B 2.907(3) . ?
Mo2 O6 2.291(4) . ?
Mo2 O7 1.766(5) . ?
Mo2 O12 2.043(5) . ?
Mo2 O21 2.099(5) . ?
Mo2 O26 1.823(5) . ?
Mo2 O35 1.683(6) . ?
Mo2B Mo12 3.198(3) . ?
Mo2B O6 2.348(5) . ?
Mo2B O7 2.315(6) . ?
Mo2B O12 1.793(5) . ?
Mo2B O21 1.566(6) . ?
Mo2B O26 2.109(5) . ?
Mo2B O35 1.736(6) . ?
Mo3 Mo3B 0.615(2) . ?
Mo3 O2 2.319(5) . ?
Mo3 O9 2.068(5) . ?
Mo3 O18 1.790(5) . ?
Mo3 O28 2.064(6) . ?
Mo3 O36 1.655(6) . ?
Mo3 O37 1.821(5) . ?
Mo3B O2 2.182(6) . ?
Mo3B O9 1.733(6) . ?
Mo3B O18 2.231(6) . ?
Mo3B O28 1.575(7) . ?
Mo3B O36 1.855(7) . ?
Mo3B O37 2.162(6) . ?
Mo4 Mo4B 0.641(2) . ?
Mo4 O4 2.285(5) . ?
Mo4 O5 2.126(5) . ?
Mo4 O21 1.741(5) . ?
Mo4 O22 2.029(5) . ?
Mo4 O24 1.715(5) . ?
Mo4 O27 1.825(5) . ?
Mo4B Mo7 3.078(3) . ?
Mo4B O4 2.351(5) . ?
Mo4B O5 1.625(6) . ?
Mo4B O21 2.271(6) . ?
Mo4B O22 1.728(5) . ?
Mo4B O24 1.707(6) . ?
Mo4B O27 2.194(6) . ?
Mo5 O2 2.281(5) . ?
Mo5 O23 1.960(5) . ?
Mo5 O30 1.684(5) . ?
Mo5 O31 1.865(5) . ?
Mo5 O32 1.899(5) . ?
Mo5 O37 1.985(5) . ?
Mo6 Mo6B 0.611(2) . ?
Mo6 O6 2.328(5) . ?
Mo6 O7 2.076(5) . ?
Mo6 O10 2.077(5) . ?
Mo6 O20 1.810(5) . ?
Mo6 O23 1.795(5) . ?
Mo6 O25 1.668(5) . ?
Mo6B O6 2.205(5) . ?
Mo6B O7 1.616(6) . ?
Mo6B O10 1.707(6) . ?
Mo6B O20 2.179(6) . ?
Mo6B O23 2.215(6) . ?
Mo6B O25 1.857(6) . ?
Mo7 O3 1.985(5) . ?
Mo7 O4 2.278(5) . ?
Mo7 O5 1.884(5) . ?
Mo7 O8 1.893(5) . ?
Mo7 O13 1.964(5) . ?
Mo7 O34 1.683(5) . ?
Mo8 O10 1.862(5) . ?
Mo8 O15 1.690(5) . ?
Mo8 O16 2.299(5) . ?
Mo8 O19 1.886(5) . ?
Mo8 O29 1.981(5) . ?
Mo8 O31 1.978(5) . ?
Mo9 Mo9B 0.623(2) . ?
Mo9 O8 2.059(5) . ?
Mo9 O16 2.281(5) . ?
Mo9 O17 1.755(6) . ?
Mo9 O29 1.801(5) . ?
Mo9 O38 2.104(5) . ?
Mo9 O40 1.714(6) . ?
Mo9B Mo10 3.124(3) . ?
Mo9B O8 1.763(6) . ?
Mo9B O16 2.390(5) . ?
Mo9B O17 2.262(6) . ?
Mo9B O29 2.177(6) . ?
Mo9B O38 1.638(6) . ?
Mo9B O40 1.659(6) . ?
Mo10 O16 2.275(5) . ?
Mo10 O19 1.972(5) . ?
Mo10 O22 1.887(5) . ?
Mo10 O26 1.959(5) . ?
Mo10 O33 1.681(5) . ?
Mo10 O38 1.881(5) . ?
Mo11 O3 1.888(5) . ?
Mo11 O4 2.290(5) . ?
Mo11 O9 1.870(5) . ?
Mo11 O11 1.989(5) . ?
Mo11 O27 1.966(5) . ?
Mo11 O39 1.692(5) . ?
Mo12 O6 2.267(4) . ?
Mo12 O11 1.861(5) . ?
Mo12 O12 1.879(5) . ?
Mo12 O14 1.703(5) . ?
Mo12 O18 1.953(5) . ?
Mo12 O20 1.989(5) . ?
Cu1 N1 1.963(6) . ?
Cu1 N2 1.967(6) . ?
Cu1 O2W 2.437(6) . ?
Cu1 O42 1.955(5) . ?
Cu1 O43 1.986(5) . ?
Cu2 N3 1.982(6) . ?
Cu2 N3 1.982(6) 3_666 ?
Cu2 O3W 2.426(7) 3_666 ?
Cu2 O3W 2.426(7) . ?
Cu2 O45 1.979(5) . ?
Cu2 O45 1.979(5) 3_666 ?
Cu3 N4 1.962(7) . ?
Cu3 N5 1.957(7) . ?
Cu3 O48 1.906(6) . ?
Cu3 O49 1.979(6) . ?
N1 C1 1.335(10) . ?
N1 C5 1.339(9) . ?
N2 C7 1.335(10) . ?
N2 C11 1.336(9) . ?
N3 C13 1.333(9) . ?
N3 C17 1.344(9) . ?
N4 C19 1.337(12) . ?
N4 C23 1.342(12) . ?
N5 C25 1.335(10) . ?
N5 C29 1.339(11) . ?
O41 C6 1.226(9) . ?
O42 C6 1.300(9) . ?
O43 C12 1.274(9) . ?
O44 C12 1.231(9) . ?
O45 C18 1.270(9) . ?
O46 C18 1.253(9) . ?
O47 C24 1.238(12) . ?
O48 C24 1.327(12) . ?
O49 C30 1.291(10) . ?
O50 C30 1.253(10) . ?
C1 H1 0.9500 . ?
C1 C2 1.383(11) . ?
C2 H2 0.9500 . ?
C2 C3 1.397(11) . ?
C3 H3 0.9500 . ?
C3 C4 1.371(11) . ?
C4 H4 0.9500 . ?
C4 C5 1.396(10) . ?
C5 C6 1.488(10) . ?
C7 H7 0.9500 . ?
C7 C8 1.372(12) . ?
C8 H8 0.9500 . ?
C8 C9 1.360(12) . ?
C9 H9 0.9500 . ?
C9 C10 1.386(11) . ?
C10 H10 0.9500 . ?
C10 C11 1.373(11) . ?
C11 C12 1.503(11) . ?
C13 H13 0.9500 . ?
C13 C14 1.391(11) . ?
C14 H14 0.9500 . ?
C14 C15 1.380(11) . ?
C15 H15 0.9500 . ?
C15 C16 1.373(11) . ?
C16 H16 0.9500 . ?
C16 C17 1.392(10) . ?
C17 C18 1.494(10) . ?
C19 H19 0.9500 . ?
C19 C20 1.415(13) . ?
C20 H20 0.9500 . ?
C20 C21 1.381(15) . ?
C21 H21 0.9500 . ?
C21 C22 1.355(15) . ?
C22 H22 0.9500 . ?
C22 C23 1.392(13) . ?
C23 C24 1.490(14) . ?
C25 H25 0.9500 . ?
C25 C26 1.381(12) . ?
C26 H26 0.9500 . ?
C26 C27 1.368(13) . ?
C27 H27 0.9500 . ?
C27 C28 1.374(12) . ?
C28 H28 0.9500 . ?
C28 C29 1.373(12) . ?
C29 C30 1.492(12) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
La1B La1 O4W 145.6(3) . . ?
La1B La1 O5W 79.4(3) . . ?
La1B La1 O6W 124.1(3) . . ?
La1B La1 O7W 64.3(3) . . ?
La1B La1 O8W 16.2(3) . . ?
La1B La1 O14 73.5(2) . . ?
La1B La1 O44 73.9(3) . . ?
La1B La1 O46 95.7(3) . . ?
La1B La1 O50 140.0(3) . . ?
O4W La1 O6W 67.7(2) . . ?
O4W La1 O7W 98.5(2) . . ?
O4W La1 O14 130.42(19) . . ?
O5W La1 O4W 66.2(2) . . ?
O5W La1 O6W 103.8(3) . . ?
O5W La1 O7W 63.0(2) . . ?
O5W La1 O14 132.5(2) . . ?
O6W La1 O14 123.7(2) . . ?
O7W La1 O6W 68.2(3) . . ?
O7W La1 O14 131.0(2) . . ?
O8W La1 O4W 137.7(2) . . ?
O8W La1 O5W 74.5(2) . . ?
O8W La1 O6W 140.0(3) . . ?
O8W La1 O7W 76.3(2) . . ?
O8W La1 O14 68.6(2) . . ?
O44 La1 O4W 133.3(2) . . ?
O44 La1 O5W 137.4(2) . . ?
O44 La1 O6W 67.2(2) . . ?
O44 La1 O7W 75.6(2) . . ?
O44 La1 O8W 86.9(2) . . ?
O44 La1 O14 69.57(17) . . ?
O46 La1 O4W 73.7(2) . . ?
O46 La1 O5W 71.62(19) . . ?
O46 La1 O6W 139.0(2) . . ?
O46 La1 O7W 132.7(2) . . ?
O46 La1 O8W 79.6(2) . . ?
O46 La1 O14 73.10(16) . . ?
O46 La1 O44 142.67(18) . . ?
O50 La1 O4W 70.1(2) . . ?
O50 La1 O5W 130.8(2) . . ?
O50 La1 O6W 78.8(3) . . ?
O50 La1 O7W 146.9(2) . . ?
O50 La1 O8W 133.2(2) . . ?
O50 La1 O14 66.59(18) . . ?
O50 La1 O44 89.7(2) . . ?
O50 La1 O46 75.46(19) . . ?
La1 La1B O5W 83.5(3) . . ?
La1 La1B O7W 98.8(3) . . ?
La1 La1B O8W 157.1(4) . . ?
La1 La1B O14 89.9(3) . . ?
La1 La1B O44 88.5(3) . . ?
La1 La1B O46 67.8(2) . . ?
O5W La1B O14 140.1(2) . . ?
O5W La1B O46 69.1(2) . . ?
O7W La1B O5W 66.6(2) . . ?
O7W La1B O14 153.1(2) . . ?
O7W La1B O44 81.8(2) . . ?
O7W La1B O46 134.9(2) . . ?
O8W La1B O5W 88.8(3) . . ?
O8W La1B O7W 97.8(3) . . ?
O8W La1B O14 82.3(3) . . ?
O8W La1B O44 109.4(3) . . ?
O8W La1B O46 89.3(3) . . ?
O14 La1B O46 71.93(18) . . ?
O44 La1B O5W 145.7(2) . . ?
O44 La1B O14 72.93(19) . . ?
O44 La1B O46 137.1(2) . . ?
O4 Ge1 O2 109.8(2) . . ?
O4 Ge1 O6 109.4(2) . . ?
O4 Ge1 O16 109.3(2) . . ?
O6 Ge1 O2 109.2(2) . . ?
O16 Ge1 O2 109.8(2) . . ?
O16 Ge1 O6 109.3(2) . . ?
Mo1B Mo1 Mo3B 134.2(3) . . ?
Mo1B Mo1 O1 79.8(4) . . ?
Mo1B Mo1 O2 91.3(3) . . ?
Mo1B Mo1 O13 112.9(3) . . ?
Mo1B Mo1 O17 31.1(3) . . ?
Mo1B Mo1 O28 144.5(3) . . ?
Mo1B Mo1 O32 56.1(3) . . ?
O1 Mo1 Mo3B 134.1(3) . . ?
O1 Mo1 O2 166.5(3) . . ?
O1 Mo1 O13 104.6(3) . . ?
O1 Mo1 O17 95.3(3) . . ?
O1 Mo1 O28 105.0(3) . . ?
O1 Mo1 O32 95.3(3) . . ?
O2 Mo1 Mo3B 48.54(14) . . ?
O13 Mo1 Mo3B 89.90(18) . . ?
O13 Mo1 O2 88.1(2) . . ?
O13 Mo1 O17 83.0(2) . . ?
O13 Mo1 O32 155.4(2) . . ?
O17 Mo1 Mo3B 129.94(15) . . ?
O17 Mo1 O2 81.63(19) . . ?
O28 Mo1 Mo3B 29.16(18) . . ?
O28 Mo1 O2 76.6(2) . . ?
O28 Mo1 O13 100.1(2) . . ?
O28 Mo1 O17 157.8(2) . . ?
O28 Mo1 O32 88.3(2) . . ?
O32 Mo1 Mo3B 86.38(16) . . ?
O32 Mo1 O2 71.33(18) . . ?
O32 Mo1 O17 80.8(2) . . ?
Mo1 Mo1B Mo5 100.7(3) . . ?
Mo1 Mo1B O1 77.9(4) . . ?
Mo1 Mo1B O2 72.6(3) . . ?
Mo1 Mo1B O13 50.7(3) . . ?
Mo1 Mo1B O17 136.4(4) . . ?
Mo1 Mo1B O28 26.2(3) . . ?
Mo1 Mo1B O32 105.8(4) . . ?
O1 Mo1B Mo5 134.9(2) . . ?
O1 Mo1B O2 148.9(3) . . ?
O1 Mo1B O13 91.2(3) . . ?
O1 Mo1B O28 84.2(3) . . ?
O1 Mo1B O32 106.1(3) . . ?
O2 Mo1B Mo5 45.23(12) . . ?
O13 Mo1B Mo5 123.14(18) . . ?
O13 Mo1B O2 77.9(2) . . ?
O13 Mo1B O28 75.3(2) . . ?
O17 Mo1B Mo5 93.8(2) . . ?
O17 Mo1B O1 118.4(4) . . ?
O17 Mo1B O2 90.3(3) . . ?
O17 Mo1B O13 87.0(3) . . ?
O17 Mo1B O28 151.9(3) . . ?
O17 Mo1B O32 107.1(3) . . ?
O28 Mo1B Mo5 78.52(15) . . ?
O28 Mo1B O2 64.98(19) . . ?
O32 Mo1B Mo5 30.06(17) . . ?
O32 Mo1B O2 73.3(2) . . ?
O32 Mo1B O13 147.9(3) . . ?
O32 Mo1B O28 79.7(2) . . ?
Mo2B Mo2 Mo6B 132.2(3) . . ?
Mo2B Mo2 O6 87.4(3) . . ?
Mo2B Mo2 O7 146.5(3) . . ?
Mo2B Mo2 O12 58.1(3) . . ?
Mo2B Mo2 O21 26.9(3) . . ?
Mo2B Mo2 O26 108.7(3) . . ?
Mo2B Mo2 O35 84.2(4) . . ?
O6 Mo2 Mo6B 48.44(13) . . ?
O7 Mo2 Mo6B 29.27(17) . . ?
O7 Mo2 O6 76.5(2) . . ?
O7 Mo2 O12 88.7(2) . . ?
O7 Mo2 O21 157.7(2) . . ?
O7 Mo2 O26 100.0(2) . . ?
O12 Mo2 Mo6B 86.57(15) . . ?
O12 Mo2 O6 70.83(17) . . ?
O12 Mo2 O21 81.04(19) . . ?
O21 Mo2 Mo6B 129.59(14) . . ?
O21 Mo2 O6 81.48(17) . . ?
O26 Mo2 Mo6B 89.55(16) . . ?
O26 Mo2 O6 87.99(19) . . ?
O26 Mo2 O12 154.7(2) . . ?
O26 Mo2 O21 82.3(2) . . ?
O35 Mo2 Mo6B 134.7(2) . . ?
O35 Mo2 O6 166.8(2) . . ?
O35 Mo2 O7 105.4(3) . . ?
O35 Mo2 O12 96.0(2) . . ?
O35 Mo2 O21 95.3(3) . . ?
O35 Mo2 O26 104.3(2) . . ?
Mo2 Mo2B Mo12 101.8(3) . . ?
Mo2 Mo2B O6 77.2(3) . . ?
Mo2 Mo2B O7 24.9(3) . . ?
Mo2 Mo2B O12 104.6(4) . . ?
Mo2 Mo2B O21 142.7(4) . . ?
Mo2 Mo2B O26 54.9(3) . . ?
Mo2 Mo2B O35 74.7(4) . . ?
O6 Mo2B Mo12 45.10(12) . . ?
O7 Mo2B Mo12 78.68(14) . . ?
O7 Mo2B O6 66.17(18) . . ?
O12 Mo2B Mo12 30.20(16) . . ?
O12 Mo2B O6 73.6(2) . . ?
O12 Mo2B O7 80.0(2) . . ?
O12 Mo2B O26 150.3(3) . . ?
O21 Mo2B Mo12 94.7(2) . . ?
O21 Mo2B O6 92.1(2) . . ?
O21 Mo2B O7 155.1(3) . . ?
O21 Mo2B O12 106.3(3) . . ?
O21 Mo2B O26 88.3(2) . . ?
O21 Mo2B O35 116.5(3) . . ?
O26 Mo2B Mo12 125.28(17) . . ?
O26 Mo2B O6 80.23(19) . . ?
O26 Mo2B O7 76.7(2) . . ?
O35 Mo2B Mo12 133.0(2) . . ?
O35 Mo2B O6 150.1(3) . . ?
O35 Mo2B O7 84.0(3) . . ?
O35 Mo2B O12 104.0(3) . . ?
O35 Mo2B O26 91.7(3) . . ?
Mo3B Mo3 O2 69.5(3) . . ?
Mo3B Mo3 O9 49.5(4) . . ?
Mo3B Mo3 O18 129.4(4) . . ?
Mo3B Mo3 O28 31.8(4) . . ?
Mo3B Mo3 O36 99.2(4) . . ?
Mo3B Mo3 O37 116.0(4) . . ?
O9 Mo3 O2 81.28(18) . . ?
O18 Mo3 O2 86.7(2) . . ?
O18 Mo3 O9 84.2(2) . . ?
O18 Mo3 O28 154.5(2) . . ?
O18 Mo3 O37 97.9(2) . . ?
O28 Mo3 O2 70.50(19) . . ?
O28 Mo3 O9 81.2(2) . . ?
O36 Mo3 O2 165.5(3) . . ?
O36 Mo3 O9 98.4(3) . . ?
O36 Mo3 O18 107.8(3) . . ?
O36 Mo3 O28 95.1(3) . . ?
O36 Mo3 O37 104.3(3) . . ?
O37 Mo3 O2 74.28(19) . . ?
O37 Mo3 O9 155.3(2) . . ?
O37 Mo3 O28 87.0(2) . . ?
Mo3 Mo3B Mo1 134.7(4) . . ?
Mo3 Mo3B O2 95.2(4) . . ?
Mo3 Mo3B O9 114.9(4) . . ?
Mo3 Mo3B O18 38.3(3) . . ?
Mo3 Mo3B O28 136.3(5) . . ?
Mo3 Mo3B O36 61.8(4) . . ?
Mo3 Mo3B O37 49.2(3) . . ?
O2 Mo3B Mo1 51.24(14) . . ?
O2 Mo3B O18 80.3(2) . . ?
O9 Mo3B Mo1 98.5(2) . . ?
O9 Mo3B O2 93.3(2) . . ?
O9 Mo3B O18 80.7(2) . . ?
O9 Mo3B O36 104.2(3) . . ?
O9 Mo3B O37 154.4(3) . . ?
O18 Mo3B Mo1 131.52(18) . . ?
O28 Mo3B Mo1 33.4(2) . . ?
O28 Mo3B O2 83.3(3) . . ?
O28 Mo3B O9 108.7(3) . . ?
O28 Mo3B O18 161.6(3) . . ?
O28 Mo3B O36 106.7(3) . . ?
O28 Mo3B O37 90.2(3) . . ?
O36 Mo3B Mo1 139.6(3) . . ?
O36 Mo3B O2 155.3(3) . . ?
O36 Mo3B O18 85.4(3) . . ?
O36 Mo3B O37 85.9(3) . . ?
O37 Mo3B Mo1 87.86(17) . . ?
O37 Mo3B O2 71.3(2) . . ?
O37 Mo3B O18 76.6(2) . . ?
Mo4B Mo4 O4 88.0(3) . . ?
Mo4B Mo4 O5 32.9(3) . . ?
Mo4B Mo4 O21 140.2(3) . . ?
Mo4B Mo4 O22 53.7(3) . . ?
Mo4B Mo4 O24 78.5(4) . . ?
Mo4B Mo4 O27 117.2(3) . . ?
O5 Mo4 O4 70.83(17) . . ?
O21 Mo4 O4 89.97(19) . . ?
O21 Mo4 O5 157.9(2) . . ?
O21 Mo4 O22 86.7(2) . . ?
O21 Mo4 O27 100.5(2) . . ?
O22 Mo4 O4 82.38(18) . . ?
O22 Mo4 O5 80.20(19) . . ?
O24 Mo4 O4 163.3(3) . . ?
O24 Mo4 O5 92.6(3) . . ?
O24 Mo4 O21 106.7(3) . . ?
O24 Mo4 O22 97.1(2) . . ?
O24 Mo4 O27 101.9(2) . . ?
O27 Mo4 O4 75.48(19) . . ?
O27 Mo4 O5 85.5(2) . . ?
O27 Mo4 O22 156.6(2) . . ?
Mo4 Mo4B Mo7 117.2(3) . . ?
Mo4 Mo4B O4 76.2(3) . . ?
Mo4 Mo4B O5 134.8(4) . . ?
Mo4 Mo4B O21 29.4(3) . . ?
Mo4 Mo4B O22 109.0(4) . . ?
Mo4 Mo4B O24 79.9(4) . . ?
Mo4 Mo4B O27 47.7(3) . . ?
O4 Mo4B Mo7 47.31(12) . . ?
O5 Mo4B Mo7 31.12(17) . . ?
O5 Mo4B O4 77.8(2) . . ?
O5 Mo4B O21 153.6(3) . . ?
O5 Mo4B O22 105.9(3) . . ?
O5 Mo4B O24 113.8(3) . . ?
O5 Mo4B O27 88.2(2) . . ?
O21 Mo4B Mo7 124.11(15) . . ?
O21 Mo4B O4 76.80(18) . . ?
O22 Mo4B Mo7 95.03(19) . . ?
O22 Mo4B O4 87.1(2) . . ?
O22 Mo4B O21 79.7(2) . . ?
O22 Mo4B O27 148.2(3) . . ?
O24 Mo4B Mo7 143.6(3) . . ?
O24 Mo4B O4 154.1(3) . . ?
O24 Mo4B O21 87.1(3) . . ?
O24 Mo4B O22 110.0(3) . . ?
O24 Mo4B O27 88.7(3) . . ?
O27 Mo4B Mo7 82.49(15) . . ?
O27 Mo4B O4 67.90(18) . . ?
O27 Mo4B O21 75.8(2) . . ?
O2 Mo5 Mo1B 47.73(13) . . ?
O23 Mo5 Mo1B 131.05(15) . . ?
O23 Mo5 O2 84.31(18) . . ?
O23 Mo5 O37 85.9(2) . . ?
O30 Mo5 Mo1B 127.5(2) . . ?
O30 Mo5 O2 168.6(2) . . ?
O30 Mo5 O23 101.4(2) . . ?
O30 Mo5 O31 103.0(2) . . ?
O30 Mo5 O32 100.1(2) . . ?
O30 Mo5 O37 98.0(2) . . ?
O31 Mo5 Mo1B 83.11(16) . . ?
O31 Mo5 O2 87.07(19) . . ?
O31 Mo5 O23 85.6(2) . . ?
O31 Mo5 O32 94.1(2) . . ?
O31 Mo5 O37 158.5(2) . . ?
O32 Mo5 Mo1B 27.78(15) . . ?
O32 Mo5 O2 73.63(19) . . ?
O32 Mo5 O23 157.9(2) . . ?
O32 Mo5 O37 86.5(2) . . ?
O37 Mo5 Mo1B 87.61(16) . . ?
O37 Mo5 O2 72.40(19) . . ?
Mo6B Mo6 O6 70.9(3) . . ?
Mo6B Mo6 O7 35.2(3) . . ?
Mo6B Mo6 O10 45.7(3) . . ?
Mo6B Mo6 O20 119.8(4) . . ?
Mo6B Mo6 O23 126.7(4) . . ?
Mo6B Mo6 O25 98.2(4) . . ?
O7 Mo6 O6 70.35(18) . . ?
O10 Mo6 O6 81.31(18) . . ?
O10 Mo6 O7 80.90(19) . . ?
O20 Mo6 O6 74.80(18) . . ?
O20 Mo6 O7 87.1(2) . . ?
O20 Mo6 O10 155.7(2) . . ?
O23 Mo6 O6 86.74(19) . . ?
O23 Mo6 O7 154.3(2) . . ?
O23 Mo6 O10 84.4(2) . . ?
O23 Mo6 O20 98.3(2) . . ?
O25 Mo6 O6 164.9(3) . . ?
O25 Mo6 O7 94.7(3) . . ?
O25 Mo6 O10 98.8(3) . . ?
O25 Mo6 O20 103.1(3) . . ?
O25 Mo6 O23 108.4(3) . . ?
Mo6 Mo6B Mo2 131.1(4) . . ?
Mo6 Mo6B O6 93.9(4) . . ?
Mo6 Mo6B O7 132.3(4) . . ?
Mo6 Mo6B O10 119.4(4) . . ?
Mo6 Mo6B O20 46.1(3) . . ?
Mo6 Mo6B O23 40.5(3) . . ?
Mo6 Mo6B O25 62.8(4) . . ?
O6 Mo6B Mo2 51.03(13) . . ?
O6 Mo6B O23 80.55(19) . . ?
O7 Mo6B Mo2 32.30(19) . . ?
O7 Mo6B O6 82.0(2) . . ?
O7 Mo6B O10 108.3(3) . . ?
O7 Mo6B O20 88.7(2) . . ?
O7 Mo6B O23 160.1(3) . . ?
O7 Mo6B O25 105.5(3) . . ?
O10 Mo6B Mo2 98.3(2) . . ?
O10 Mo6B O6 93.8(2) . . ?
O10 Mo6B O20 155.7(3) . . ?
O10 Mo6B O23 82.3(2) . . ?
O10 Mo6B O25 106.4(3) . . ?
O20 Mo6B Mo2 86.84(15) . . ?
O20 Mo6B O6 71.03(19) . . ?
O20 Mo6B O23 76.7(2) . . ?
O23 Mo6B Mo2 131.58(17) . . ?
O25 Mo6B Mo2 137.1(2) . . ?
O25 Mo6B O6 154.5(3) . . ?
O25 Mo6B O20 84.6(3) . . ?
O25 Mo6B O23 86.8(3) . . ?
O3 Mo7 Mo4B 86.66(15) . . ?
O3 Mo7 O4 73.65(18) . . ?
O4 Mo7 Mo4B 49.36(12) . . ?
O5 Mo7 Mo4B 26.47(16) . . ?
O5 Mo7 O3 89.1(2) . . ?
O5 Mo7 O4 75.22(19) . . ?
O5 Mo7 O8 93.6(2) . . ?
O5 Mo7 O13 158.9(2) . . ?
O8 Mo7 Mo4B 86.91(15) . . ?
O8 Mo7 O3 159.8(2) . . ?
O8 Mo7 O4 87.71(19) . . ?
O8 Mo7 O13 84.7(2) . . ?
O13 Mo7 Mo4B 132.60(15) . . ?
O13 Mo7 O3 85.7(2) . . ?
O13 Mo7 O4 83.71(18) . . ?
O34 Mo7 Mo4B 126.91(19) . . ?
O34 Mo7 O3 97.2(2) . . ?
O34 Mo7 O4 169.7(2) . . ?
O34 Mo7 O5 100.4(2) . . ?
O34 Mo7 O8 102.0(2) . . ?
O34 Mo7 O13 100.5(2) . . ?
O10 Mo8 O16 86.93(19) . . ?
O10 Mo8 O19 93.2(2) . . ?
O10 Mo8 O29 158.3(2) . . ?
O10 Mo8 O31 85.1(2) . . ?
O15 Mo8 O10 103.6(2) . . ?
O15 Mo8 O16 169.1(2) . . ?
O15 Mo8 O19 102.1(2) . . ?
O15 Mo8 O29 97.2(2) . . ?
O15 Mo8 O31 100.1(2) . . ?
O19 Mo8 O16 74.25(19) . . ?
O19 Mo8 O29 88.2(2) . . ?
O19 Mo8 O31 157.6(2) . . ?
O29 Mo8 O16 72.62(18) . . ?
O31 Mo8 O16 83.31(19) . . ?
O31 Mo8 O29 85.4(2) . . ?
Mo9B Mo9 O8 53.7(3) . . ?
Mo9B Mo9 O16 92.4(3) . . ?
Mo9B Mo9 O17 138.9(4) . . ?
Mo9B Mo9 O29 119.7(4) . . ?
Mo9B Mo9 O38 35.6(3) . . ?
Mo9B Mo9 O40 74.4(4) . . ?
O8 Mo9 O16 82.81(18) . . ?
O8 Mo9 O38 79.61(19) . . ?
O17 Mo9 O8 86.1(2) . . ?
O17 Mo9 O16 90.0(2) . . ?
O17 Mo9 O29 100.7(2) . . ?
O17 Mo9 O38 157.0(2) . . ?
O29 Mo9 O8 157.9(2) . . ?
O29 Mo9 O16 76.2(2) . . ?
O29 Mo9 O38 86.7(2) . . ?
O38 Mo9 O16 70.53(18) . . ?
O40 Mo9 O8 95.6(3) . . ?
O40 Mo9 O16 164.4(3) . . ?
O40 Mo9 O17 105.5(3) . . ?
O40 Mo9 O29 102.7(3) . . ?
O40 Mo9 O38 93.9(3) . . ?
Mo9 Mo9B Mo10 112.8(3) . . ?
Mo9 Mo9B O8 109.8(4) . . ?
Mo9 Mo9B O16 72.5(3) . . ?
Mo9 Mo9B O17 30.7(3) . . ?
Mo9 Mo9B O29 45.9(3) . . ?
Mo9 Mo9B O38 131.6(4) . . ?
Mo9 Mo9B O40 84.4(4) . . ?
O8 Mo9B Mo10 93.46(19) . . ?
O8 Mo9B O16 86.2(2) . . ?
O8 Mo9B O17 79.9(2) . . ?
O8 Mo9B O29 147.9(3) . . ?
O16 Mo9B Mo10 46.42(13) . . ?
O17 Mo9B Mo10 122.80(17) . . ?
O17 Mo9B O16 76.39(19) . . ?
O29 Mo9B Mo10 82.03(15) . . ?
O29 Mo9B O16 67.62(19) . . ?
O29 Mo9B O17 76.2(2) . . ?
O38 Mo9B Mo10 29.54(18) . . ?
O38 Mo9B O8 103.1(3) . . ?
O38 Mo9B O16 75.5(2) . . ?
O38 Mo9B O17 151.4(3) . . ?
O38 Mo9B O29 88.5(3) . . ?
O38 Mo9B O40 116.4(3) . . ?
O40 Mo9B Mo10 144.6(3) . . ?
O40 Mo9B O8 110.1(3) . . ?
O40 Mo9B O16 155.4(3) . . ?
O40 Mo9B O17 88.1(3) . . ?
O40 Mo9B O29 90.3(3) . . ?
O16 Mo10 Mo9B 49.54(13) . . ?
O19 Mo10 Mo9B 85.86(15) . . ?
O19 Mo10 O16 73.30(18) . . ?
O22 Mo10 Mo9B 87.00(15) . . ?
O22 Mo10 O16 87.03(19) . . ?
O22 Mo10 O19 158.9(2) . . ?
O22 Mo10 O26 84.5(2) . . ?
O26 Mo10 Mo9B 133.35(15) . . ?
O26 Mo10 O16 84.22(18) . . ?
O26 Mo10 O19 86.1(2) . . ?
O33 Mo10 Mo9B 125.32(19) . . ?
O33 Mo10 O16 170.9(2) . . ?
O33 Mo10 O19 99.8(2) . . ?
O33 Mo10 O22 100.5(2) . . ?
O33 Mo10 O26 101.3(2) . . ?
O33 Mo10 O38 99.9(2) . . ?
O38 Mo10 Mo9B 25.43(16) . . ?
O38 Mo10 O16 74.53(19) . . ?
O38 Mo10 O19 88.9(2) . . ?
O38 Mo10 O22 93.1(2) . . ?
O38 Mo10 O26 158.7(2) . . ?
O3 Mo11 O4 75.09(18) . . ?
O3 Mo11 O11 158.6(2) . . ?
O3 Mo11 O27 88.4(2) . . ?
O9 Mo11 O3 93.1(2) . . ?
O9 Mo11 O4 86.78(19) . . ?
O9 Mo11 O11 84.9(2) . . ?
O9 Mo11 O27 158.5(2) . . ?
O11 Mo11 O4 83.50(18) . . ?
O27 Mo11 O4 72.89(18) . . ?
O27 Mo11 O11 85.86(19) . . ?
O39 Mo11 O3 102.4(2) . . ?
O39 Mo11 O4 170.2(2) . . ?
O39 Mo11 O9 102.9(2) . . ?
O39 Mo11 O11 98.8(2) . . ?
O39 Mo11 O27 97.7(2) . . ?
O6 Mo12 Mo2B 47.19(12) . . ?
O11 Mo12 Mo2B 82.63(15) . . ?
O11 Mo12 O6 87.13(19) . . ?
O11 Mo12 O12 92.9(2) . . ?
O11 Mo12 O18 86.0(2) . . ?
O11 Mo12 O20 159.5(2) . . ?
O12 Mo12 Mo2B 28.69(15) . . ?
O12 Mo12 O6 74.21(18) . . ?
O12 Mo12 O18 158.2(2) . . ?
O12 Mo12 O20 87.2(2) . . ?
O14 Mo12 Mo2B 130.50(19) . . ?
O14 Mo12 O6 168.9(2) . . ?
O14 Mo12 O11 103.6(2) . . ?
O14 Mo12 O12 102.1(2) . . ?
O14 Mo12 O18 99.4(2) . . ?
O14 Mo12 O20 96.4(2) . . ?
O18 Mo12 Mo2B 130.12(16) . . ?
O18 Mo12 O6 83.95(19) . . ?
O18 Mo12 O20 86.4(2) . . ?
O20 Mo12 Mo2B 87.84(15) . . ?
O20 Mo12 O6 73.18(18) . . ?
N1 Cu1 N2 175.5(3) . . ?
N1 Cu1 O2W 91.3(2) . . ?
N1 Cu1 O43 97.3(2) . . ?
N2 Cu1 O2W 93.3(2) . . ?
N2 Cu1 O43 82.5(2) . . ?
O42 Cu1 N1 83.6(2) . . ?
O42 Cu1 N2 96.5(2) . . ?
O42 Cu1 O2W 87.9(2) . . ?
O42 Cu1 O43 177.7(3) . . ?
O43 Cu1 O2W 94.2(2) . . ?
N3 Cu2 N3 180.0 . 3_666 ?
N3 Cu2 O3W 86.1(3) 3_666 . ?
N3 Cu2 O3W 93.9(3) . . ?
N3 Cu2 O3W 93.9(3) 3_666 3_666 ?
N3 Cu2 O3W 86.1(3) . 3_666 ?
O3W Cu2 O3W 180.00(15) 3_666 . ?
O45 Cu2 N3 82.8(2) . . ?
O45 Cu2 N3 97.2(2) . 3_666 ?
O45 Cu2 N3 97.2(2) 3_666 . ?
O45 Cu2 N3 82.8(2) 3_666 3_666 ?
O45 Cu2 O3W 87.9(2) . 3_666 ?
O45 Cu2 O3W 92.1(2) 3_666 3_666 ?
O45 Cu2 O3W 92.1(2) . . ?
O45 Cu2 O3W 87.9(2) 3_666 . ?
O45 Cu2 O45 180.0 3_666 . ?
N4 Cu3 O49 98.2(3) . . ?
N5 Cu3 N4 178.9(3) . . ?
N5 Cu3 O49 82.7(3) . . ?
O48 Cu3 N4 85.3(3) . . ?
O48 Cu3 N5 93.8(3) . . ?
O48 Cu3 O49 176.5(3) . . ?
C1 N1 Cu1 129.0(5) . . ?
C1 N1 C5 118.6(6) . . ?
C5 N1 Cu1 112.1(5) . . ?
C7 N2 Cu1 128.5(6) . . ?
C7 N2 C11 118.3(7) . . ?
C11 N2 Cu1 113.1(5) . . ?
C13 N3 Cu2 127.8(5) . . ?
C13 N3 C17 120.1(6) . . ?
C17 N3 Cu2 112.0(5) . . ?
C19 N4 Cu3 129.2(7) . . ?
C19 N4 C23 119.1(8) . . ?
C23 N4 Cu3 111.7(6) . . ?
C25 N5 Cu3 127.5(6) . . ?
C25 N5 C29 118.7(7) . . ?
C29 N5 Cu3 113.8(5) . . ?
La1B O5W La1 17.16(8) . . ?
La1B O7W La1 16.97(9) . . ?
La1B O8W La1 6.74(12) . . ?
Mo1 O1 Mo1B 22.30(12) . . ?
Ge1 O2 Mo1 123.1(2) . . ?
Ge1 O2 Mo1B 119.1(2) . . ?
Ge1 O2 Mo3 122.4(2) . . ?
Ge1 O2 Mo3B 123.7(3) . . ?
Ge1 O2 Mo5 122.0(2) . . ?
Mo1 O2 Mo1B 16.07(7) . . ?
Mo1 O2 Mo3 93.03(17) . . ?
Mo1 O2 Mo5 96.42(17) . . ?
Mo3 O2 Mo1B 106.44(19) . . ?
Mo3B O2 Mo1 80.22(18) . . ?
Mo3B O2 Mo1B 94.9(2) . . ?
Mo3B O2 Mo3 15.30(8) . . ?
Mo3B O2 Mo5 101.7(2) . . ?
Mo5 O2 Mo1B 87.04(17) . . ?
Mo5 O2 Mo3 92.10(17) . . ?
Mo11 O3 Mo7 118.0(2) . . ?
Ge1 O4 Mo4 121.7(2) . . ?
Ge1 O4 Mo4B 124.7(2) . . ?
Ge1 O4 Mo7 122.7(2) . . ?
Ge1 O4 Mo11 122.8(2) . . ?
Mo4 O4 Mo4B 15.81(7) . . ?
Mo4 O4 Mo11 91.54(17) . . ?
Mo7 O4 Mo4 97.06(17) . . ?
Mo7 O4 Mo4B 83.33(16) . . ?
Mo7 O4 Mo11 93.25(17) . . ?
Mo11 O4 Mo4B 100.11(19) . . ?
Mo4B O5 Mo4 12.35(11) . . ?
Mo4B O5 Mo7 122.4(3) . . ?
Mo7 O5 Mo4 116.8(2) . . ?
Ge1 O6 Mo2 123.3(2) . . ?
Ge1 O6 Mo2B 118.5(2) . . ?
Ge1 O6 Mo6 122.8(2) . . ?
Ge1 O6 Mo6B 123.1(2) . . ?
Ge1 O6 Mo12 122.4(2) . . ?
Mo2 O6 Mo2B 15.47(7) . . ?
Mo2 O6 Mo6 92.63(17) . . ?
Mo6 O6 Mo2B 106.06(19) . . ?
Mo6B O6 Mo2 80.53(17) . . ?
Mo6B O6 Mo2B 95.1(2) . . ?
Mo6B O6 Mo6 15.17(7) . . ?
Mo6B O6 Mo12 101.85(19) . . ?
Mo12 O6 Mo2 95.79(17) . . ?
Mo12 O6 Mo2B 87.72(17) . . ?
Mo12 O6 Mo6 91.62(16) . . ?
Mo2 O7 Mo2B 8.60(9) . . ?
Mo2 O7 Mo6 120.5(3) . . ?
Mo6 O7 Mo2B 116.5(2) . . ?
Mo6B O7 Mo2 118.4(3) . . ?
Mo6B O7 Mo2B 116.3(3) . . ?
Mo6B O7 Mo6 12.57(12) . . ?
Mo7 O8 Mo9 147.9(3) . . ?
Mo9B O8 Mo7 162.7(3) . . ?
Mo9B O8 Mo9 16.53(10) . . ?
Mo3B O9 Mo3 15.64(11) . . ?
Mo3B O9 Mo11 159.3(3) . . ?
Mo11 O9 Mo3 151.0(3) . . ?
Mo6B O10 Mo6 14.84(10) . . ?
Mo6B O10 Mo8 159.0(3) . . ?
Mo8 O10 Mo6 150.6(3) . . ?
Mo12 O11 Mo11 151.6(3) . . ?
Mo2B O12 Mo2 17.26(10) . . ?
Mo2B O12 Mo12 121.1(3) . . ?
Mo12 O12 Mo2 119.1(2) . . ?
Mo1 O13 Mo1B 16.34(9) . . ?
Mo1 O13 Mo7 156.9(3) . . ?
Mo7 O13 Mo1B 143.1(3) . . ?
La1B O14 La1 16.56(8) . . ?
Mo12 O14 La1 168.0(3) . . ?
Mo12 O14 La1B 151.4(3) . . ?
Ge1 O16 Mo8 122.8(2) . . ?
Ge1 O16 Mo9 121.6(2) . . ?
Ge1 O16 Mo9B 124.4(2) . . ?
Ge1 O16 Mo10 123.0(2) . . ?
Mo8 O16 Mo9B 99.51(19) . . ?
Mo9 O16 Mo8 91.15(17) . . ?
Mo9 O16 Mo9B 15.09(7) . . ?
Mo10 O16 Mo8 93.32(17) . . ?
Mo10 O16 Mo9 97.05(18) . . ?
Mo10 O16 Mo9B 84.04(17) . . ?
Mo1 O17 Mo9B 143.8(3) . . ?
Mo1B O17 Mo1 12.49(13) . . ?
Mo1B O17 Mo9 164.2(4) . . ?
Mo1B O17 Mo9B 156.3(3) . . ?
Mo9 O17 Mo1 152.3(3) . . ?
Mo9 O17 Mo9B 10.42(9) . . ?
Mo3 O18 Mo3B 12.28(9) . . ?
Mo3 O18 Mo12 156.3(3) . . ?
Mo12 O18 Mo3B 144.0(3) . . ?
Mo8 O19 Mo10 119.1(2) . . ?
Mo6 O20 Mo6B 14.08(8) . . ?
Mo6 O20 Mo12 120.2(2) . . ?
Mo12 O20 Mo6B 112.7(2) . . ?
Mo2 O21 Mo4B 143.4(2) . . ?
Mo2B O21 Mo2 10.43(12) . . ?
Mo2B O21 Mo4 162.1(3) . . ?
Mo2B O21 Mo4B 153.7(3) . . ?
Mo4 O21 Mo2 152.6(3) . . ?
Mo4 O21 Mo4B 10.40(9) . . ?
Mo4B O22 Mo4 17.38(10) . . ?
Mo4B O22 Mo10 163.7(3) . . ?
Mo10 O22 Mo4 148.6(3) . . ?
Mo5 O23 Mo6B 143.1(3) . . ?
Mo6 O23 Mo5 155.8(3) . . ?
Mo6 O23 Mo6B 12.76(9) . . ?
Mo4B O24 Mo4 21.58(10) . . ?
Mo6 O25 Mo6B 19.00(10) . . ?
Mo2 O26 Mo2B 16.34(8) . . ?
Mo2 O26 Mo10 156.7(3) . . ?
Mo10 O26 Mo2B 142.7(3) . . ?
Mo4 O27 Mo4B 15.05(8) . . ?
Mo4 O27 Mo11 119.6(2) . . ?
Mo11 O27 Mo4B 117.5(2) . . ?
Mo1 O28 Mo1B 9.38(9) . . ?
Mo1 O28 Mo3 119.9(3) . . ?
Mo3 O28 Mo1B 116.9(2) . . ?
Mo3B O28 Mo1 117.4(3) . . ?
Mo3B O28 Mo1B 116.6(3) . . ?
Mo3B O28 Mo3 11.86(13) . . ?
Mo8 O29 Mo9B 118.7(2) . . ?
Mo9 O29 Mo8 119.7(3) . . ?
Mo9 O29 Mo9B 14.39(9) . . ?
Mo5 O31 Mo8 152.4(3) . . ?
Mo1B O32 Mo1 18.02(10) . . ?
Mo1B O32 Mo5 122.2(3) . . ?
Mo5 O32 Mo1 118.6(2) . . ?
Mo2 O35 Mo2B 21.05(10) . . ?
Mo3 O36 Mo3B 19.09(11) . . ?
Mo3 O37 Mo3B 14.80(9) . . ?
Mo3 O37 Mo5 121.0(3) . . ?
Mo5 O37 Mo3B 113.2(2) . . ?
Mo9B O38 Mo9 12.78(12) . . ?
Mo9B O38 Mo10 125.0(3) . . ?
Mo10 O38 Mo9 117.8(2) . . ?
Mo9B O40 Mo9 21.20(11) . . ?
C6 O42 Cu1 113.9(5) . . ?
C12 O43 Cu1 113.7(5) . . ?
La1B O44 La1 17.61(8) . . ?
C12 O44 La1 144.0(5) . . ?
C12 O44 La1B 146.2(5) . . ?
C18 O45 Cu2 114.2(5) . . ?
La1 O46 La1B 16.49(7) . . ?
C18 O46 La1 143.3(5) . . ?
C18 O46 La1B 145.4(5) . . ?
C24 O48 Cu3 112.8(6) . . ?
C30 O49 Cu3 113.6(5) . . ?
C30 O50 La1 147.1(6) . . ?
N1 C1 H1 118.8 . . ?
N1 C1 C2 122.5(8) . . ?
C2 C1 H1 118.8 . . ?
C1 C2 H2 120.5 . . ?
C1 C2 C3 119.0(7) . . ?
C3 C2 H2 120.5 . . ?
C2 C3 H3 120.8 . . ?
C4 C3 C2 118.4(7) . . ?
C4 C3 H3 120.8 . . ?
C3 C4 H4 120.3 . . ?
C3 C4 C5 119.3(7) . . ?
C5 C4 H4 120.3 . . ?
N1 C5 C4 122.1(7) . . ?
N1 C5 C6 115.1(6) . . ?
C4 C5 C6 122.8(7) . . ?
O41 C6 O42 123.0(7) . . ?
O41 C6 C5 121.9(7) . . ?
O42 C6 C5 115.1(6) . . ?
N2 C7 H7 119.0 . . ?
N2 C7 C8 122.1(8) . . ?
C8 C7 H7 119.0 . . ?
C7 C8 H8 120.2 . . ?
C9 C8 C7 119.6(8) . . ?
C9 C8 H8 120.2 . . ?
C8 C9 H9 120.5 . . ?
C8 C9 C10 118.9(8) . . ?
C10 C9 H9 120.5 . . ?
C9 C10 H10 120.8 . . ?
C11 C10 C9 118.4(8) . . ?
C11 C10 H10 120.8 . . ?
N2 C11 C10 122.6(7) . . ?
N2 C11 C12 113.9(6) . . ?
C10 C11 C12 123.4(7) . . ?
O43 C12 C11 116.1(7) . . ?
O44 C12 O43 124.1(7) . . ?
O44 C12 C11 119.8(7) . . ?
N3 C13 H13 119.6 . . ?
N3 C13 C14 120.9(7) . . ?
C14 C13 H13 119.6 . . ?
C13 C14 H14 120.3 . . ?
C15 C14 C13 119.4(7) . . ?
C15 C14 H14 120.3 . . ?
C14 C15 H15 120.3 . . ?
C16 C15 C14 119.3(7) . . ?
C16 C15 H15 120.3 . . ?
C15 C16 H16 120.5 . . ?
C15 C16 C17 118.9(7) . . ?
C17 C16 H16 120.5 . . ?
N3 C17 C16 121.3(7) . . ?
N3 C17 C18 114.8(6) . . ?
C16 C17 C18 123.9(6) . . ?
O45 C18 C17 116.1(6) . . ?
O46 C18 O45 125.5(7) . . ?
O46 C18 C17 118.4(6) . . ?
N4 C19 H19 119.7 . . ?
N4 C19 C20 120.6(10) . . ?
C20 C19 H19 119.7 . . ?
C19 C20 H20 120.3 . . ?
C21 C20 C19 119.5(10) . . ?
C21 C20 H20 120.3 . . ?
C20 C21 H21 120.4 . . ?
C22 C21 C20 119.2(10) . . ?
C22 C21 H21 120.4 . . ?
C21 C22 H22 120.4 . . ?
C21 C22 C23 119.3(10) . . ?
C23 C22 H22 120.4 . . ?
N4 C23 C22 122.4(9) . . ?
N4 C23 C24 113.9(8) . . ?
C22 C23 C24 123.6(10) . . ?
O47 C24 O48 121.1(10) . . ?
O47 C24 C23 122.7(10) . . ?
O48 C24 C23 116.2(9) . . ?
N5 C25 H25 119.2 . . ?
N5 C25 C26 121.6(9) . . ?
C26 C25 H25 119.2 . . ?
C25 C26 H26 120.4 . . ?
C27 C26 C25 119.1(9) . . ?
C27 C26 H26 120.4 . . ?
C26 C27 H27 120.2 . . ?
C26 C27 C28 119.7(9) . . ?
C28 C27 H27 120.2 . . ?
C27 C28 H28 120.9 . . ?
C27 C28 C29 118.3(9) . . ?
C29 C28 H28 120.9 . . ?
N5 C29 C28 122.6(8) . . ?
N5 C29 C30 113.7(7) . . ?
C28 C29 C30 123.7(8) . . ?
O49 C30 C29 116.2(8) . . ?
O50 C30 O49 123.3(9) . . ?
O50 C30 C29 120.5(8) . . ?

_smtbx_masks_special_details     ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 0.116 0.055 0.466 17.2 7.8 ?
2 0.116 0.445 0.966 17.2 7.7 ?
3 0.500 0.000 0.500 359.9 81.8 ?
4 0.500 0.500 0.000 359.9 81.8 ?
5 0.884 0.555 0.034 17.2 7.3 ?
6 0.884 0.945 0.534 17.2 7.3 ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_database_code_depnum_ccdc_archive 'CCDC 1940344'
loop_
_audit_author_name
_audit_author_address
'Jun-Wei Zhao'
;Henan University
China
;
_audit_update_record             
;
2019-09-07 deposited with the CCDC.	2019-09-23 downloaded from the CCDC.
;

# start Validation Reply Form

_vrf_PLAT975_2                   
;
PROBLEM:  Check Calcd Resid. Dens.  1.05A   From O8W      1.98 eA-3  
RESPONSE: Due to the large structure and the existence of a large 
 amount of weight atoms, the intensity data are not very good, 
leading to the ADP max/min ratio of some water molecules, and it is 
very difficult to refine this large structure, therefore, 
 in the final refinement, the MO, Ge, Cu and La atoms were refined 
anisotropically, some O atoms and water molecules were
 refined isotropically. Thus, the isotropical refinement and the isotropic 
atomic displacement parameter restriction of O8W leads to
 the occurrence of a residual density near to O8W.
;

_vrf_PLAT201_2                   
;
PROBLEM: Isotropic non-H Atoms in Main Residue(s) .......    2 Report 
RESPONSE: Due to the large structure and the existence of a large 
 amount of weight atoms, the intensity data are not very good, 
 leading to the ADP max/min ratio of some water molecules, and it is 
very difficult to refine this large structure, therefore, 
 in the final refinement, the MO, Ge, Cu and Ce atoms were refined 
anisotropically, some O atoms and water molecules were
 refined isotropically.
;

_vrf_PLAT306_2                   
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) ....... O9W Check
RESPONSE: The hydrogen atoms of the water molecules could not be directly 
 located from the difference Fourier maps because of the presence of too many
 heavy atoms in the structure.
;

_vrf_PLAT430_2                   
;
PROBLEM: Short Inter D...A Contact O1W ..O9W . 2.80 Ang.
RESPONSE: In the crystal structure, there are a number of short contacts between 
Ow(H2O) and O(POM) or Ow(H2O) in the range of 2.61-2.89 Ang, which indicate 
extensive hydrogen bonding interactions among them. 
;

# end Validation Reply Form



_audit_creation_date             2019-09-07
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        
;
 ? 
;
_chemical_formula_moiety         
'C60 H40 Ce2 Cu5 Ge2 Mo24 N10 O112, 2(N), 16(O)'
_chemical_formula_sum            'C60 H124 Ce2 Cu5 Ge2 Mo24 N12 O139'
_chemical_formula_weight         6283.38
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P2(1)/c '
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   19.4634(5)
_cell_length_b                   14.4095(3)
_cell_length_c                   28.9976(6)
_cell_angle_alpha                90
_cell_angle_beta                 101.2040(10)
_cell_angle_gamma                90
_cell_volume                     7977.6(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9868
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      28.20
_cell_measurement_theta_min      2.54
_shelx_estimated_absorpt_T_max   0.348
_shelx_estimated_absorpt_T_min   0.272
_exptl_absorpt_coefficient_mu    3.519
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4782
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1268 before and 0.0728 after correction.
The Ratio of minimum to maximum transmission is 0.6413.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            green
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    2.616
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             6026
_exptl_crystal_preparation       ?
_exptl_crystal_size_max          0.5
_exptl_crystal_size_mid          0.5
_exptl_crystal_size_min          0.38
_exptl_special_details           
;
 ? 
;
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0598
_diffrn_reflns_av_unetI/netI     0.0462
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            74035
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_min         2.143
_diffrn_ambient_temperature      150.0
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    ?
_reflns_Friedel_fraction_max     ?
_reflns_number_gt                11106
_reflns_number_total             13993
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         2.702
_refine_diff_density_min         -2.276
_refine_diff_density_rms         0.179
_refine_ls_extinction_coef       0.00010(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.067
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1058
_refine_ls_number_reflns         13993
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0675
_refine_ls_R_factor_gt           0.0510
_refine_ls_restrained_S_all      1.067
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0533P)²+65.5640P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1208
_refine_ls_wR_factor_ref         0.1289
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Others
 Fixed Sof: Ce1(0.85) Ce1'(0.15) Mo1(0.75) Mo1'(0.25) Mo2(0.75) Mo2'(0.25)
 Mo3(0.75) Mo3'(0.25) Mo4(0.75) Mo4'(0.25) Mo6(0.75) Mo6'(0.25) Mo9(0.75)
 Mo9'(0.25)
 Fixed Uiso: O7W(0.05479) O8W(0.06857)
3.a Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C3(H3), C4(H4), C7(H7), C8(H8), C9(H9), C10(H10), C13(H13),
 C14(H14), C15(H15), C16(H16), C19(H19), C20(H20), C21(H21), C22(H22), C25(H25),
  C26(H26), C27(H27), C28(H28)
;
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     iterative
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ce1 Ce 0.20906(3) 0.34608(5) 0.46644(2) 0.02544(15) Uani 0.85 1 d . . . . .
Ce1' Ce 0.21772(15) 0.2894(2) 0.47623(10) 0.0156(6) Uiso 0.15 1 d . . . . .
Ge1 Ge 0.25675(4) 0.00673(5) 0.26606(3) 0.01589(18) Uani 1 1 d . . . . .
Mo1 Mo 0.43693(5) -0.04112(10) 0.27539(4) 0.0284(2) Uani 0.75 1 d . . . . .
Mo1' Mo 0.42767(16) -0.0870(2) 0.27191(10) 0.0147(7) Uiso 0.25 1 d . . . . .
Mo2 Mo 0.07949(5) 0.05760(9) 0.26919(4) 0.0209(2) Uani 0.75 1 d . . . . .
Mo2' Mo 0.08671(16) 0.0946(2) 0.26217(10) 0.0093(7) Uiso 0.25 1 d . . . . .
Mo3 Mo 0.39040(6) 0.08802(7) 0.35931(5) 0.0245(2) Uani 0.75 1 d . . . . .
Mo3' Mo 0.40207(19) 0.0880(2) 0.34301(12) 0.0164(9) Uiso 0.25 1 d . . . . .
Mo4 Mo 0.17164(5) 0.16391(7) 0.18091(4) 0.0216(2) Uani 0.75 1 d . . . . .
Mo4' Mo 0.18173(15) 0.1419(2) 0.16434(10) 0.0106(7) Uiso 0.25 1 d . . . . .
Mo5 Mo 0.35026(4) -0.13639(5) 0.35510(3) 0.03198(19) Uani 1 1 d . . . . .
Mo6 Mo 0.17244(7) -0.05877(7) 0.35994(5) 0.0233(2) Uani 0.75 1 d . . . . .
Mo6' Mo 0.14944(16) -0.0674(2) 0.34233(11) 0.0108(8) Uiso 0.25 1 d . . . . .
Mo7 Mo 0.33740(4) 0.09152(5) 0.17579(3) 0.0314(2) Uani 1 1 d . . . . .
Mo8 Mo 0.20269(4) -0.22838(5) 0.26511(3) 0.02887(18) Uani 1 1 d . . . . .
Mo9 Mo 0.29802(6) -0.16355(7) 0.18922(5) 0.0218(2) Uani 0.75 1 d . . . . .
Mo9' Mo 0.28107(19) -0.1489(2) 0.17140(12) 0.0187(9) Uiso 0.25 1 d . . . . .
Mo10 Mo 0.12861(4) -0.09175(5) 0.17677(3) 0.02868(18) Uani 1 1 d . . . . .
Mo11 Mo 0.30678(4) 0.24099(5) 0.25670(2) 0.02541(18) Uani 1 1 d . . . . .
Mo12 Mo 0.20733(4) 0.16208(5) 0.34734(2) 0.02643(18) Uani 1 1 d . . . . .
Cu1 Cu -0.08192(5) 0.27003(7) 0.49271(3) 0.0262(2) Uani 1 1 d . . . . .
Cu2 Cu 0.500000 0.500000 0.500000 0.0239(3) Uani 1 2 d S T P . .
Cu3 Cu 0.25411(6) 0.50338(7) 0.27627(4) 0.0348(3) Uani 1 1 d . . . . .
N1 N -0.0776(4) 0.3257(5) 0.5552(2) 0.0268(15) Uani 1 1 d . . . . .
N2 N -0.0838(4) 0.2061(5) 0.4322(2) 0.0257(15) Uani 1 1 d . . . . .
N3 N 0.4920(3) 0.4482(5) 0.4364(2) 0.0238(15) Uani 1 1 d . . . . .
N4 N 0.3428(5) 0.5686(5) 0.2824(3) 0.047(2) Uani 1 1 d . . . . .
N5 N 0.1646(4) 0.4374(5) 0.2695(3) 0.0333(17) Uani 1 1 d . . . . .
N6 N 0.3538(6) 0.7655(7) 0.0346(3) 0.067(3) Uani 1 1 d . . . . .
O1W O -0.0348(4) 0.1173(5) 0.5392(3) 0.056(2) Uani 1 1 d . . . . .
O2W O -0.1333(4) 0.4115(4) 0.4532(2) 0.0471(18) Uani 1 1 d . . . . .
O3W O 0.4501(4) 0.6474(6) 0.4706(3) 0.076(3) Uani 1 1 d . . . . .
O4W O 0.2439(4) 0.5157(5) 0.4834(3) 0.0548(19) Uani 1 1 d . . . . .
O5W O 0.3011(4) 0.3675(5) 0.5414(2) 0.054(2) Uani 1 1 d . . . . .
O6W O 0.1052(5) 0.4478(6) 0.4797(4) 0.085(3) Uani 1 1 d . . . . .
O7W O 0.1735(4) 0.3064(5) 0.5448(3) 0.055 Uiso 1 1 d . . . . .
O8W O 0.2613(5) 0.1894(6) 0.4864(3) 0.069 Uiso 1 1 d . . . . .
O9W O 1.1107(5) 1.3606(7) 0.0552(4) 0.091(3) Uani 1 1 d . . . . .
O10W O -0.2483(7) 0.0683(9) 0.4766(5) 0.125(4) Uiso 1 1 d . . . . .
O11W O 0.7245(4) 0.4070(6) 0.4328(3) 0.066(2) Uani 1 1 d . . . . .
O12W O 0.6855(4) 1.0948(4) 0.0785(2) 0.0461(17) Uani 1 1 d . . . . .
O13W O 1.2271(7) 1.3872(7) 0.1294(4) 0.107(4) Uani 1 1 d . . . . .
O17W O 0.6798(7) 0.8082(9) 0.4192(5) 0.129(4) Uiso 1 1 d . . . . .
O1 O 0.5128(3) -0.0832(6) 0.2634(2) 0.059(2) Uani 1 1 d . . . . .
O2 O 0.3364(3) -0.0165(3) 0.30266(18) 0.0210(11) Uani 1 1 d . . . . .
O3 O 0.3572(3) 0.2116(4) 0.20920(18) 0.0222(12) Uani 1 1 d . . . . .
O4 O 0.2657(3) 0.0984(3) 0.22897(17) 0.0176(11) Uani 1 1 d . . . . .
O5 O 0.2522(3) 0.1421(4) 0.14242(18) 0.0255(12) Uani 1 1 d . . . . .
O6 O 0.1961(3) 0.0362(3) 0.29996(17) 0.0167(11) Uani 1 1 d . . . . .
O7 O 0.0785(3) -0.0156(4) 0.31812(19) 0.0269(13) Uani 1 1 d . . . . .
O8 O 0.3077(3) -0.0318(3) 0.16379(18) 0.0211(11) Uani 1 1 d . . . . .
O9 O 0.3701(3) 0.1767(4) 0.30311(18) 0.0235(12) Uani 1 1 d . . . . .
O10 O 0.1634(3) -0.1579(3) 0.30703(19) 0.0241(12) Uani 1 1 d . . . . .
O11 O 0.2396(3) 0.2247(3) 0.29942(17) 0.0188(11) Uani 1 1 d . . . . .
O12 O 0.1144(3) 0.1633(3) 0.31472(17) 0.0195(11) Uani 1 1 d . . . . .
O13 O 0.4047(3) 0.0388(4) 0.22819(18) 0.0240(12) Uani 1 1 d . . . . .
O14 O 0.2069(3) 0.2446(3) 0.38898(17) 0.0231(12) Uani 1 1 d . . . . .
O15 O 0.1874(3) -0.3390(4) 0.2797(2) 0.0289(13) Uani 1 1 d . . . . .
O16 O 0.2288(3) -0.0903(3) 0.23284(17) 0.0188(11) Uani 1 1 d . . . . .
O17 O 0.3715(3) -0.1360(4) 0.2322(2) 0.0298(14) Uani 1 1 d . . . . .
O18 O 0.3035(3) 0.1179(3) 0.36680(18) 0.0236(12) Uani 1 1 d . . . . .
O19 O 0.1274(3) -0.2052(3) 0.21466(18) 0.0230(12) Uani 1 1 d . . . . .
O20 O 0.1805(3) 0.0569(3) 0.38459(18) 0.0217(12) Uani 1 1 d . . . . .
O21 O 0.1212(3) 0.1441(4) 0.2234(2) 0.0265(13) Uani 1 1 d . . . . .
O22 O 0.1526(3) 0.0295(4) 0.16133(18) 0.0223(12) Uani 1 1 d . . . . .
O23 O 0.2627(3) -0.0895(3) 0.37112(18) 0.0242(12) Uani 1 1 d . . . . .
O24 O 0.1182(3) 0.2143(4) 0.1343(2) 0.0453(17) Uani 1 1 d . . . . .
O25 O 0.1336(4) -0.1175(4) 0.3970(2) 0.0444(18) Uani 1 1 d . . . . .
O26 O 0.0876(3) -0.0295(3) 0.22540(17) 0.0193(11) Uani 1 1 d . . . . .
O27 O 0.2241(3) 0.2623(4) 0.20714(18) 0.0218(12) Uani 1 1 d . . . . .
O28 O 0.4628(3) 0.0382(4) 0.3223(2) 0.0354(15) Uani 1 1 d . . . . .
O29 O 0.2609(3) -0.2567(4) 0.2183(2) 0.0266(13) Uani 1 1 d . . . . .
O30 O 0.3751(3) -0.2140(4) 0.3983(2) 0.0373(15) Uani 1 1 d . . . . .
O31 O 0.2921(3) -0.2064(3) 0.30879(19) 0.0235(12) Uani 1 1 d . . . . .
O32 O 0.4283(3) -0.1416(4) 0.3249(2) 0.0326(14) Uani 1 1 d . . . . .
O33 O 0.0568(3) -0.1109(4) 0.13474(19) 0.0289(13) Uani 1 1 d . . . . .
O34 O 0.3894(3) 0.1077(4) 0.13651(19) 0.0296(13) Uani 1 1 d . . . . .
O35 O -0.0040(3) 0.0967(5) 0.2531(2) 0.0465(18) Uani 1 1 d . . . . .
O36 O 0.4461(3) 0.1530(4) 0.3959(2) 0.0468(18) Uani 1 1 d . . . . .
O37 O 0.3951(3) -0.0252(4) 0.38871(18) 0.0260(12) Uani 1 1 d . . . . .
O38 O 0.1974(3) -0.1469(4) 0.14813(19) 0.0255(13) Uani 1 1 d . . . . .
O39 O 0.3281(3) 0.3526(4) 0.26802(19) 0.0271(13) Uani 1 1 d . . . . .
O40 O 0.3296(4) -0.2205(4) 0.1457(3) 0.0468(18) Uani 1 1 d . . . . .
O41 O -0.2513(3) 0.2511(4) 0.5479(2) 0.0329(14) Uani 1 1 d . . . . .
O42 O -0.1761(3) 0.2345(4) 0.49966(19) 0.0284(13) Uani 1 1 d . . . . .
O43 O 0.0146(3) 0.3020(4) 0.4857(2) 0.0326(14) Uani 1 1 d . . . . .
O44 O 0.0935(3) 0.2655(5) 0.4428(2) 0.0482(19) Uani 1 1 d . . . . .
O45 O 0.4055(3) 0.4434(4) 0.49495(18) 0.0257(13) Uani 1 1 d . . . . .
O46 O 0.3245(3) 0.3652(4) 0.4442(2) 0.0309(14) Uani 1 1 d . . . . .
O47 O 0.3162(5) 0.5528(7) 0.1591(3) 0.076(3) Uani 1 1 d . . . . .
O48 O 0.2497(4) 0.5079(5) 0.2104(2) 0.0524(19) Uani 1 1 d . . . . .
O49 O 0.2502(3) 0.4928(4) 0.3441(2) 0.0414(16) Uani 1 1 d . . . . .
O50 O 0.1840(4) 0.4378(4) 0.3927(2) 0.0452(17) Uani 1 1 d . . . . .
C1 C -0.0230(5) 0.3683(6) 0.5834(3) 0.0305(19) Uani 1 1 d . . . . .
H1 H 0.018498 0.380303 0.571709 0.037 Uiso 1 1 calc R . . . .
C2 C -0.0261(5) 0.3945(6) 0.6288(3) 0.032(2) Uani 1 1 d . . . . .
H2 H 0.012324 0.425565 0.647726 0.038 Uiso 1 1 calc R . . . .
C3 C -0.0863(4) 0.3749(5) 0.6465(3) 0.0264(18) Uani 1 1 d . . . . .
H3 H -0.088771 0.390177 0.677979 0.032 Uiso 1 1 calc R . . . .
C4 C -0.1419(4) 0.3332(5) 0.6174(3) 0.0243(18) Uani 1 1 d . . . . .
H4 H -0.183973 0.321042 0.628363 0.029 Uiso 1 1 calc R . . . .
C5 C -0.1363(4) 0.3089(5) 0.5719(3) 0.0216(17) Uani 1 1 d . . . . .
C6 C -0.1932(4) 0.2620(6) 0.5390(3) 0.0274(19) Uani 1 1 d . . . . .
C7 C -0.1373(5) 0.1653(6) 0.4043(3) 0.033(2) Uani 1 1 d . . . . .
H7 H -0.181972 0.166897 0.412904 0.040 Uiso 1 1 calc R . . . .
C8 C -0.1306(5) 0.1207(7) 0.3636(3) 0.037(2) Uani 1 1 d . . . . .
H8 H -0.169886 0.092019 0.344243 0.044 Uiso 1 1 calc R . . . .
C9 C -0.0650(5) 0.1187(7) 0.3513(3) 0.037(2) Uani 1 1 d . . . . .
H9 H -0.058352 0.087381 0.323625 0.045 Uiso 1 1 calc R . . . .
C10 C -0.0106(5) 0.1624(6) 0.3796(3) 0.035(2) Uani 1 1 d . . . . .
H10 H 0.034489 0.162922 0.371575 0.042 Uiso 1 1 calc R . . . .
C11 C -0.0212(4) 0.2054(5) 0.4197(3) 0.0252(18) Uani 1 1 d . . . . .
C12 C 0.0342(4) 0.2615(6) 0.4513(3) 0.0287(19) Uani 1 1 d . . . . .
C13 C 0.5392(4) 0.4507(6) 0.4084(3) 0.033(2) Uani 1 1 d . . . . .
H13 H 0.582861 0.480536 0.419100 0.039 Uiso 1 1 calc R . . . .
C14 C 0.5258(5) 0.4106(7) 0.3639(3) 0.036(2) Uani 1 1 d . . . . .
H14 H 0.560000 0.413185 0.344676 0.043 Uiso 1 1 calc R . . . .
C15 C 0.4629(5) 0.3672(6) 0.3480(3) 0.032(2) Uani 1 1 d . . . . .
H15 H 0.453121 0.339383 0.317761 0.038 Uiso 1 1 calc R . . . .
C16 C 0.4138(5) 0.3647(6) 0.3768(3) 0.0293(19) Uani 1 1 d . . . . .
H16 H 0.369623 0.335828 0.366501 0.035 Uiso 1 1 calc R . . . .
C17 C 0.4307(4) 0.4056(5) 0.4211(3) 0.0227(17) Uani 1 1 d . . . . .
C18 C 0.3821(4) 0.4045(6) 0.4555(3) 0.0240(18) Uani 1 1 d . . . . .
C19 C 0.3865(5) 0.5973(7) 0.3215(4) 0.050(3) Uani 1 1 d . . . . .
H19 H 0.375458 0.585859 0.351490 0.060 Uiso 1 1 calc R . . . .
C20 C 0.4484(5) 0.6442(7) 0.3179(4) 0.051(3) Uani 1 1 d . . . . .
H20 H 0.479890 0.663970 0.345444 0.061 Uiso 1 1 calc R . . . .
C21 C 0.4633(5) 0.6615(7) 0.2737(5) 0.057(3) Uani 1 1 d . . . . .
H21 H 0.504632 0.694439 0.271150 0.068 Uiso 1 1 calc R . . . .
C22 C 0.4197(6) 0.6322(8) 0.2345(5) 0.059(3) Uani 1 1 d . . . . .
H22 H 0.429320 0.643817 0.204133 0.071 Uiso 1 1 calc R . . . .
C23 C 0.3591(5) 0.5836(6) 0.2405(4) 0.043(3) Uani 1 1 d . . . . .
C24 C 0.3073(6) 0.5481(8) 0.1998(4) 0.054(3) Uani 1 1 d . . . . .
C25 C 0.1237(5) 0.4097(6) 0.2300(3) 0.036(2) Uani 1 1 d . . . . .
H25 H 0.137123 0.422572 0.200847 0.043 Uiso 1 1 calc R . . . .
C26 C 0.0617(5) 0.3622(7) 0.2300(4) 0.046(3) Uani 1 1 d . . . . .
H26 H 0.032803 0.343245 0.201329 0.056 Uiso 1 1 calc R . . . .
C27 C 0.0424(5) 0.3427(6) 0.2730(4) 0.043(2) Uani 1 1 d . . . . .
H27 H 0.000868 0.308751 0.273938 0.052 Uiso 1 1 calc R . . . .
C28 C 0.0831(5) 0.3725(6) 0.3129(4) 0.038(2) Uani 1 1 d . . . . .
H28 H 0.069553 0.362176 0.342182 0.046 Uiso 1 1 calc R . . . .
C29 C 0.1450(5) 0.4183(6) 0.3112(3) 0.034(2) Uani 1 1 d . . . . .
C30 C 0.1952(5) 0.4517(6) 0.3522(3) 0.036(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ce1 Ce1' 0.871(3) . ?
Ce1 O4W 2.559(7) . ?
Ce1 O5W 2.553(7) . ?
Ce1 O6W 2.586(8) . ?
Ce1 O7W 2.567(7) . ?
Ce1 O8W 2.498(9) . ?
Ce1 O14 2.673(5) . ?
Ce1 O44 2.506(6) . ?
Ce1 O46 2.471(5) . ?
Ce1 O50 2.480(7) . ?
Ce1' O5W 2.506(7) . ?
Ce1' O7W 2.329(8) . ?
Ce1' O8W 1.669(9) . ?
Ce1' O14 2.579(5) . ?
Ce1' O44 2.448(7) . ?
Ce1' O46 2.670(6) . ?
Ge1 O2 1.732(5) . ?
Ge1 O4 1.734(5) . ?
Ge1 O6 1.730(5) . ?
Ge1 O16 1.724(5) . ?
Mo1 Mo1' 0.687(3) . ?
Mo1 Mo3' 2.878(4) . ?
Mo1 O1 1.695(6) . ?
Mo1 O2 2.277(5) . ?
Mo1 O13 1.805(5) . ?
Mo1 O17 2.106(6) . ?
Mo1 O28 1.773(7) . ?
Mo1 O32 2.067(6) . ?
Mo1' Mo5 3.164(3) . ?
Mo1' O1 1.724(7) . ?
Mo1' O2 2.367(6) . ?
Mo1' O13 2.207(6) . ?
Mo1' O17 1.590(7) . ?
Mo1' O28 2.339(7) . ?
Mo1' O32 1.723(6) . ?
Mo2 Mo2' 0.598(2) . ?
Mo2 Mo6' 2.911(3) . ?
Mo2 O6 2.292(5) . ?
Mo2 O7 1.771(6) . ?
Mo2 O12 2.044(5) . ?
Mo2 O21 2.097(6) . ?
Mo2 O26 1.814(5) . ?
Mo2 O35 1.697(6) . ?
Mo2' Mo12 3.210(3) . ?
Mo2' O6 2.353(6) . ?
Mo2' O7 2.298(6) . ?
Mo2' O12 1.809(6) . ?
Mo2' O21 1.587(6) . ?
Mo2' O26 2.085(6) . ?
Mo2' O35 1.734(7) . ?
Mo3 Mo3' 0.563(3) . ?
Mo3 O2 2.324(5) . ?
Mo3 O9 2.048(5) . ?
Mo3 O18 1.800(6) . ?
Mo3 O28 2.059(6) . ?
Mo3 O36 1.653(6) . ?
Mo3 O37 1.835(5) . ?
Mo3' O2 2.165(6) . ?
Mo3' O9 1.756(6) . ?
Mo3' O18 2.205(6) . ?
Mo3' O28 1.595(7) . ?
Mo3' O36 1.859(7) . ?
Mo3' O37 2.122(6) . ?
Mo4 Mo4' 0.638(2) . ?
Mo4 O4 2.279(5) . ?
Mo4 O5 2.117(6) . ?
Mo4 O21 1.741(6) . ?
Mo4 O22 2.032(5) . ?
Mo4 O24 1.700(6) . ?
Mo4 O27 1.825(5) . ?
Mo4' Mo7 3.070(3) . ?
Mo4' O4 2.321(6) . ?
Mo4' O5 1.620(6) . ?
Mo4' O21 2.259(6) . ?
Mo4' O22 1.712(6) . ?
Mo4' O24 1.720(7) . ?
Mo4' O27 2.199(6) . ?
Mo5 O2 2.283(5) . ?
Mo5 O23 1.970(5) . ?
Mo5 O30 1.680(6) . ?
Mo5 O31 1.874(6) . ?
Mo5 O32 1.898(6) . ?
Mo5 O37 1.987(6) . ?
Mo6 Mo6' 0.623(3) . ?
Mo6 O6 2.328(5) . ?
Mo6 O7 2.083(6) . ?
Mo6 O10 2.079(5) . ?
Mo6 O20 1.808(5) . ?
Mo6 O23 1.780(6) . ?
Mo6 O25 1.662(5) . ?
Mo6' O6 2.234(6) . ?
Mo6' O7 1.605(7) . ?
Mo6' O10 1.712(6) . ?
Mo6' O20 2.188(6) . ?
Mo6' O23 2.224(6) . ?
Mo6' O25 1.823(6) . ?
Mo7 O3 1.984(5) . ?
Mo7 O4 2.274(5) . ?
Mo7 O5 1.896(6) . ?
Mo7 O8 1.880(5) . ?
Mo7 O13 1.957(5) . ?
Mo7 O34 1.680(5) . ?
Mo8 O10 1.859(5) . ?
Mo8 O15 1.690(5) . ?
Mo8 O16 2.298(5) . ?
Mo8 O19 1.888(6) . ?
Mo8 O29 1.973(5) . ?
Mo8 O31 1.968(6) . ?
Mo9 Mo9' 0.595(3) . ?
Mo9 O8 2.059(5) . ?
Mo9 O16 2.279(5) . ?
Mo9 O17 1.751(6) . ?
Mo9 O29 1.808(5) . ?
Mo9 O38 2.099(6) . ?
Mo9 O40 1.716(6) . ?
Mo9' Mo10 3.112(4) . ?
Mo9' O8 1.792(6) . ?
Mo9' O16 2.372(6) . ?
Mo9' O17 2.245(7) . ?
Mo9' O29 2.150(6) . ?
Mo9' O38 1.637(7) . ?
Mo9' O40 1.669(7) . ?
Mo10 O16 2.284(5) . ?
Mo10 O19 1.972(5) . ?
Mo10 O22 1.885(5) . ?
Mo10 O26 1.967(5) . ?
Mo10 O33 1.688(6) . ?
Mo10 O38 1.883(5) . ?
Mo11 O3 1.888(5) . ?
Mo11 O4 2.293(5) . ?
Mo11 O9 1.882(5) . ?
Mo11 O11 1.983(5) . ?
Mo11 O27 1.962(5) . ?
Mo11 O39 1.677(5) . ?
Mo12 O6 2.261(5) . ?
Mo12 O11 1.865(5) . ?
Mo12 O12 1.871(5) . ?
Mo12 O14 1.696(5) . ?
Mo12 O18 1.953(6) . ?
Mo12 O20 1.989(5) . ?
Cu1 N1 1.968(7) . ?
Cu1 N2 1.977(7) . ?
Cu1 O42 1.950(6) . ?
Cu1 O43 1.983(5) . ?
Cu2 N3 1.967(6) . ?
Cu2 N3 1.967(6) 3_666 ?
Cu2 O3W 2.420(8) . ?
Cu2 O3W 2.420(8) 3_666 ?
Cu2 O45 1.991(5) . ?
Cu2 O45 1.991(5) 3_666 ?
Cu3 N4 1.944(9) . ?
Cu3 N5 1.961(8) . ?
Cu3 O48 1.897(7) . ?
Cu3 O49 1.988(7) . ?
N1 C1 1.356(11) . ?
N1 C5 1.346(10) . ?
N2 C7 1.324(11) . ?
N2 C11 1.337(10) . ?
N3 C13 1.340(10) . ?
N3 C17 1.338(10) . ?
N4 C19 1.344(14) . ?
N4 C23 1.331(13) . ?
N5 C25 1.323(12) . ?
N5 C29 1.366(11) . ?
O41 C6 1.219(9) . ?
O42 C6 1.312(10) . ?
O43 C12 1.276(9) . ?
O44 C12 1.228(10) . ?
O45 C18 1.276(10) . ?
O46 C18 1.241(10) . ?
O47 C24 1.227(13) . ?
O48 C24 1.348(14) . ?
O49 C30 1.286(11) . ?
O50 C30 1.252(11) . ?
C1 C2 1.381(12) . ?
C2 C3 1.396(12) . ?
C3 C4 1.374(12) . ?
C4 C5 1.391(11) . ?
C5 C6 1.476(11) . ?
C7 C8 1.373(12) . ?
C8 C9 1.391(13) . ?
C9 C10 1.363(12) . ?
C10 C11 1.369(11) . ?
C11 C12 1.508(11) . ?
C13 C14 1.389(12) . ?
C14 C15 1.372(12) . ?
C15 C16 1.384(12) . ?
C16 C17 1.394(11) . ?
C17 C18 1.503(11) . ?
C19 C20 1.403(14) . ?
C20 C21 1.390(17) . ?
C21 C22 1.348(17) . ?
C22 C23 1.410(15) . ?
C23 C24 1.486(15) . ?
C25 C26 1.387(14) . ?
C26 C27 1.398(15) . ?
C27 C28 1.338(14) . ?
C28 C29 1.382(13) . ?
C29 C30 1.464(13) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ce1' Ce1 O4W 143.8(3) . . ?
Ce1' Ce1 O5W 77.1(3) . . ?
Ce1' Ce1 O6W 126.2(3) . . ?
Ce1' Ce1 O7W 64.6(2) . . ?
Ce1' Ce1 O8W 14.5(3) . . ?
Ce1' Ce1 O14 74.4(2) . . ?
Ce1' Ce1 O44 76.2(3) . . ?
Ce1' Ce1 O46 93.5(2) . . ?
Ce1' Ce1 O50 140.8(2) . . ?
O4W Ce1 O6W 67.4(2) . . ?
O4W Ce1 O7W 98.6(2) . . ?
O4W Ce1 O14 130.10(19) . . ?
O5W Ce1 O4W 66.7(2) . . ?
O5W Ce1 O6W 104.1(3) . . ?
O5W Ce1 O7W 62.5(2) . . ?
O5W Ce1 O14 132.5(2) . . ?
O6W Ce1 O14 123.3(3) . . ?
O7W Ce1 O6W 69.0(3) . . ?
O7W Ce1 O14 131.3(2) . . ?
O8W Ce1 O4W 137.6(3) . . ?
O8W Ce1 O5W 74.0(3) . . ?
O8W Ce1 O6W 140.6(3) . . ?
O8W Ce1 O7W 76.2(3) . . ?
O8W Ce1 O14 68.9(2) . . ?
O8W Ce1 O44 87.0(3) . . ?
O44 Ce1 O4W 133.3(2) . . ?
O44 Ce1 O5W 137.1(2) . . ?
O44 Ce1 O6W 67.5(2) . . ?
O44 Ce1 O7W 75.9(2) . . ?
O44 Ce1 O14 69.51(18) . . ?
O46 Ce1 O4W 73.9(2) . . ?
O46 Ce1 O5W 71.7(2) . . ?
O46 Ce1 O6W 138.8(2) . . ?
O46 Ce1 O7W 132.2(2) . . ?
O46 Ce1 O8W 79.1(2) . . ?
O46 Ce1 O14 73.06(18) . . ?
O46 Ce1 O44 142.57(19) . . ?
O46 Ce1 O50 75.6(2) . . ?
O50 Ce1 O4W 69.9(2) . . ?
O50 Ce1 O5W 131.1(2) . . ?
O50 Ce1 O6W 78.3(3) . . ?
O50 Ce1 O7W 147.2(2) . . ?
O50 Ce1 O8W 133.2(2) . . ?
O50 Ce1 O14 66.34(19) . . ?
O50 Ce1 O44 89.7(2) . . ?
Ce1 Ce1' O5W 83.1(3) . . ?
Ce1 Ce1' O7W 95.7(3) . . ?
Ce1 Ce1' O8W 158.0(4) . . ?
Ce1 Ce1' O14 86.6(2) . . ?
Ce1 Ce1' O44 83.6(3) . . ?
Ce1 Ce1' O46 67.5(2) . . ?
O5W Ce1' O14 140.3(2) . . ?
O5W Ce1' O46 69.2(2) . . ?
O7W Ce1' O5W 66.5(3) . . ?
O7W Ce1' O14 153.0(3) . . ?
O7W Ce1' O44 81.5(3) . . ?
O7W Ce1' O46 134.1(3) . . ?
O8W Ce1' O5W 91.3(4) . . ?
O8W Ce1' O7W 101.5(4) . . ?
O8W Ce1' O14 84.2(3) . . ?
O8W Ce1' O44 112.2(4) . . ?
O8W Ce1' O46 90.6(3) . . ?
O14 Ce1' O46 71.46(18) . . ?
O44 Ce1' O5W 143.7(3) . . ?
O44 Ce1' O14 72.0(2) . . ?
O44 Ce1' O46 134.1(2) . . ?
O2 Ge1 O4 110.0(2) . . ?
O6 Ge1 O2 109.1(2) . . ?
O6 Ge1 O4 109.1(2) . . ?
O16 Ge1 O2 109.5(2) . . ?
O16 Ge1 O4 109.3(2) . . ?
O16 Ge1 O6 109.9(2) . . ?
Mo1' Mo1 Mo3' 129.2(3) . . ?
Mo1' Mo1 O1 80.8(4) . . ?
Mo1' Mo1 O2 89.0(3) . . ?
Mo1' Mo1 O13 117.3(3) . . ?
Mo1' Mo1 O17 34.7(3) . . ?
Mo1' Mo1 O28 139.4(3) . . ?
Mo1' Mo1 O32 51.3(3) . . ?
O1 Mo1 Mo3' 134.6(3) . . ?
O1 Mo1 O2 165.9(3) . . ?
O1 Mo1 O13 105.1(3) . . ?
O1 Mo1 O17 95.5(3) . . ?
O1 Mo1 O28 105.1(3) . . ?
O1 Mo1 O32 94.8(3) . . ?
O2 Mo1 Mo3' 47.95(15) . . ?
O13 Mo1 Mo3' 90.64(19) . . ?
O13 Mo1 O2 88.2(2) . . ?
O13 Mo1 O17 83.2(2) . . ?
O13 Mo1 O32 155.5(2) . . ?
O17 Mo1 Mo3' 128.99(16) . . ?
O17 Mo1 O2 81.2(2) . . ?
O28 Mo1 Mo3' 29.5(2) . . ?
O28 Mo1 O2 76.6(2) . . ?
O28 Mo1 O13 100.1(3) . . ?
O28 Mo1 O17 157.3(2) . . ?
O28 Mo1 O32 88.2(3) . . ?
O32 Mo1 Mo3' 85.32(17) . . ?
O32 Mo1 O2 71.2(2) . . ?
O32 Mo1 O17 80.6(2) . . ?
Mo1 Mo1' Mo5 104.7(3) . . ?
Mo1 Mo1' O1 76.0(4) . . ?
Mo1 Mo1' O2 74.1(3) . . ?
Mo1 Mo1' O13 46.6(3) . . ?
Mo1 Mo1' O17 131.1(4) . . ?
Mo1 Mo1' O28 29.5(3) . . ?
Mo1 Mo1' O32 110.6(4) . . ?
O1 Mo1' Mo5 136.9(3) . . ?
O1 Mo1' O2 148.6(4) . . ?
O1 Mo1' O13 89.1(3) . . ?
O1 Mo1' O28 83.9(3) . . ?
O2 Mo1' Mo5 46.02(13) . . ?
O13 Mo1' Mo5 123.33(18) . . ?
O13 Mo1' O2 77.3(2) . . ?
O13 Mo1' O28 74.2(2) . . ?
O17 Mo1' Mo5 95.2(2) . . ?
O17 Mo1' O1 117.1(4) . . ?
O17 Mo1' O2 90.2(3) . . ?
O17 Mo1' O13 85.1(3) . . ?
O17 Mo1' O28 150.6(3) . . ?
O17 Mo1' O32 109.1(3) . . ?
O28 Mo1' Mo5 79.71(16) . . ?
O28 Mo1' O2 65.3(2) . . ?
O32 Mo1' Mo5 30.69(19) . . ?
O32 Mo1' O1 107.6(3) . . ?
O32 Mo1' O2 74.7(2) . . ?
O32 Mo1' O13 148.5(3) . . ?
O32 Mo1' O28 81.0(3) . . ?
Mo2' Mo2 Mo6' 133.9(3) . . ?
Mo2' Mo2 O6 88.4(4) . . ?
Mo2' Mo2 O7 147.6(4) . . ?
Mo2' Mo2 O12 58.9(3) . . ?
Mo2' Mo2 O21 26.9(3) . . ?
Mo2' Mo2 O26 108.8(4) . . ?
Mo2' Mo2 O35 83.4(4) . . ?
O6 Mo2 Mo6' 49.12(13) . . ?
O7 Mo2 Mo6' 28.84(18) . . ?
O7 Mo2 O6 76.8(2) . . ?
O7 Mo2 O12 88.9(2) . . ?
O7 Mo2 O21 158.0(2) . . ?
O7 Mo2 O26 99.4(2) . . ?
O12 Mo2 Mo6' 86.59(15) . . ?
O12 Mo2 O6 70.67(18) . . ?
O12 Mo2 O21 81.1(2) . . ?
O21 Mo2 Mo6' 130.18(16) . . ?
O21 Mo2 O6 81.40(19) . . ?
O26 Mo2 Mo6' 89.41(18) . . ?
O26 Mo2 O6 88.0(2) . . ?
O26 Mo2 O12 154.8(2) . . ?
O26 Mo2 O21 82.6(2) . . ?
O35 Mo2 Mo6' 133.9(3) . . ?
O35 Mo2 O6 167.0(3) . . ?
O35 Mo2 O7 105.1(3) . . ?
O35 Mo2 O12 96.4(3) . . ?
O35 Mo2 O21 95.5(3) . . ?
O35 Mo2 O26 104.2(3) . . ?
Mo2 Mo2' Mo12 101.2(3) . . ?
Mo2 Mo2' O6 76.9(3) . . ?
Mo2 Mo2' O7 24.4(3) . . ?
Mo2 Mo2' O12 104.7(4) . . ?
Mo2 Mo2' O21 143.3(4) . . ?
Mo2 Mo2' O26 55.5(3) . . ?
Mo2 Mo2' O35 76.5(4) . . ?
O6 Mo2' Mo12 44.75(13) . . ?
O7 Mo2' Mo12 78.86(16) . . ?
O7 Mo2' O6 66.68(19) . . ?
O12 Mo2' Mo12 29.82(17) . . ?
O12 Mo2' O6 73.1(2) . . ?
O12 Mo2' O7 80.4(2) . . ?
O12 Mo2' O26 150.4(3) . . ?
O21 Mo2' Mo12 93.6(2) . . ?
O21 Mo2' O6 91.2(3) . . ?
O21 Mo2' O7 155.2(3) . . ?
O21 Mo2' O12 104.7(3) . . ?
O21 Mo2' O26 88.6(3) . . ?
O21 Mo2' O35 116.3(4) . . ?
O26 Mo2' Mo12 125.16(19) . . ?
O26 Mo2' O6 80.5(2) . . ?
O26 Mo2' O7 77.1(2) . . ?
O35 Mo2' Mo12 133.1(2) . . ?
O35 Mo2' O6 151.6(3) . . ?
O35 Mo2' O7 84.9(3) . . ?
O35 Mo2' O12 104.3(3) . . ?
O35 Mo2' O26 92.6(3) . . ?
Mo3' Mo3 O2 66.8(4) . . ?
Mo3' Mo3 O9 51.7(4) . . ?
Mo3' Mo3 O18 130.1(5) . . ?
Mo3' Mo3 O28 29.9(4) . . ?
Mo3' Mo3 O36 102.6(5) . . ?
Mo3' Mo3 O37 113.4(5) . . ?
O9 Mo3 O2 81.4(2) . . ?
O9 Mo3 O28 81.3(2) . . ?
O18 Mo3 O2 86.2(2) . . ?
O18 Mo3 O9 84.6(2) . . ?
O18 Mo3 O28 154.3(2) . . ?
O18 Mo3 O37 96.9(2) . . ?
O28 Mo3 O2 70.6(2) . . ?
O36 Mo3 O2 166.3(3) . . ?
O36 Mo3 O9 99.1(3) . . ?
O36 Mo3 O18 107.6(3) . . ?
O36 Mo3 O28 95.9(3) . . ?
O36 Mo3 O37 103.8(3) . . ?
O37 Mo3 O2 74.2(2) . . ?
O37 Mo3 O9 155.4(2) . . ?
O37 Mo3 O28 87.4(2) . . ?
Mo3 Mo3' Mo1 139.5(5) . . ?
Mo3 Mo3' O2 99.3(5) . . ?
Mo3 Mo3' O9 113.8(5) . . ?
Mo3 Mo3' O18 38.6(4) . . ?
Mo3 Mo3' O28 140.0(6) . . ?
Mo3 Mo3' O36 60.2(4) . . ?
Mo3 Mo3' O37 52.5(4) . . ?
O2 Mo3' Mo1 51.34(15) . . ?
O2 Mo3' O18 81.2(2) . . ?
O9 Mo3' Mo1 97.0(2) . . ?
O9 Mo3' O2 93.1(3) . . ?
O9 Mo3' O18 81.1(3) . . ?
O9 Mo3' O36 102.9(3) . . ?
O9 Mo3' O37 156.0(3) . . ?
O18 Mo3' Mo1 132.4(2) . . ?
O28 Mo3' Mo1 33.2(2) . . ?
O28 Mo3' O2 83.5(3) . . ?
O28 Mo3' O9 105.9(3) . . ?
O28 Mo3' O18 163.5(3) . . ?
O28 Mo3' O36 106.3(4) . . ?
O28 Mo3' O37 91.8(3) . . ?
O36 Mo3' Mo1 139.2(3) . . ?
O36 Mo3' O2 157.8(3) . . ?
O36 Mo3' O18 86.1(3) . . ?
O36 Mo3' O37 87.0(3) . . ?
O37 Mo3' Mo1 88.91(19) . . ?
O37 Mo3' O2 72.6(2) . . ?
O37 Mo3' O18 77.8(2) . . ?
Mo4' Mo4 O4 85.8(3) . . ?
Mo4' Mo4 O5 33.0(3) . . ?
Mo4' Mo4 O21 138.6(3) . . ?
Mo4' Mo4 O22 51.8(3) . . ?
Mo4' Mo4 O24 81.0(4) . . ?
Mo4' Mo4 O27 118.1(3) . . ?
O5 Mo4 O4 70.84(19) . . ?
O21 Mo4 O4 89.8(2) . . ?
O21 Mo4 O5 157.7(2) . . ?
O21 Mo4 O22 86.8(2) . . ?
O21 Mo4 O27 100.3(2) . . ?
O22 Mo4 O4 81.8(2) . . ?
O22 Mo4 O5 79.9(2) . . ?
O24 Mo4 O4 163.3(3) . . ?
O24 Mo4 O5 92.6(3) . . ?
O24 Mo4 O21 106.9(3) . . ?
O24 Mo4 O22 97.8(3) . . ?
O24 Mo4 O27 101.9(3) . . ?
O27 Mo4 O4 75.5(2) . . ?
O27 Mo4 O5 85.6(2) . . ?
O27 Mo4 O22 156.1(2) . . ?
Mo4 Mo4' Mo7 118.6(3) . . ?
Mo4 Mo4' O4 78.3(3) . . ?
Mo4 Mo4' O5 134.6(4) . . ?
Mo4 Mo4' O21 30.7(3) . . ?
Mo4 Mo4' O22 111.2(4) . . ?
Mo4 Mo4' O24 77.5(4) . . ?
Mo4 Mo4' O27 47.0(3) . . ?
O4 Mo4' Mo7 47.42(13) . . ?
O5 Mo4' Mo7 31.79(19) . . ?
O5 Mo4' O4 78.5(2) . . ?
O5 Mo4' O21 154.6(3) . . ?
O5 Mo4' O22 106.2(3) . . ?
O5 Mo4' O24 112.3(3) . . ?
O5 Mo4' O27 88.1(3) . . ?
O21 Mo4' Mo7 124.76(18) . . ?
O21 Mo4' O4 77.3(2) . . ?
O22 Mo4' Mo7 95.3(2) . . ?
O22 Mo4' O4 87.7(2) . . ?
O22 Mo4' O21 80.6(2) . . ?
O22 Mo4' O24 110.5(3) . . ?
O22 Mo4' O27 149.3(3) . . ?
O24 Mo4' Mo7 142.7(3) . . ?
O24 Mo4' O4 153.8(3) . . ?
O24 Mo4' O21 86.9(3) . . ?
O24 Mo4' O27 87.7(3) . . ?
O27 Mo4' Mo7 82.63(16) . . ?
O27 Mo4' O4 68.2(2) . . ?
O27 Mo4' O21 75.8(2) . . ?
O2 Mo5 Mo1' 48.25(14) . . ?
O23 Mo5 Mo1' 131.61(16) . . ?
O23 Mo5 O2 84.33(19) . . ?
O23 Mo5 O37 85.7(2) . . ?
O30 Mo5 Mo1' 127.4(2) . . ?
O30 Mo5 O2 168.8(3) . . ?
O30 Mo5 O23 100.9(3) . . ?
O30 Mo5 O31 102.9(3) . . ?
O30 Mo5 O32 100.2(3) . . ?
O30 Mo5 O37 97.8(3) . . ?
O31 Mo5 Mo1' 83.43(16) . . ?
O31 Mo5 O2 87.3(2) . . ?
O31 Mo5 O23 85.6(2) . . ?
O31 Mo5 O32 94.3(2) . . ?
O31 Mo5 O37 158.7(2) . . ?
O32 Mo5 Mo1' 27.60(17) . . ?
O32 Mo5 O2 74.0(2) . . ?
O32 Mo5 O23 158.3(2) . . ?
O32 Mo5 O37 86.8(2) . . ?
O37 Mo5 Mo1' 87.93(16) . . ?
O37 Mo5 O2 72.6(2) . . ?
Mo6' Mo6 O6 73.7(3) . . ?
Mo6' Mo6 O7 34.1(3) . . ?
Mo6' Mo6 O10 46.6(3) . . ?
Mo6' Mo6 O20 120.1(4) . . ?
Mo6' Mo6 O23 128.8(4) . . ?
Mo6' Mo6 O25 94.8(4) . . ?
O7 Mo6 O6 70.61(19) . . ?
O10 Mo6 O6 81.55(18) . . ?
O10 Mo6 O7 80.6(2) . . ?
O20 Mo6 O6 74.88(19) . . ?
O20 Mo6 O7 87.4(2) . . ?
O20 Mo6 O10 156.0(2) . . ?
O23 Mo6 O6 87.2(2) . . ?
O23 Mo6 O7 154.7(2) . . ?
O23 Mo6 O10 84.4(2) . . ?
O23 Mo6 O20 98.6(2) . . ?
O25 Mo6 O6 164.6(3) . . ?
O25 Mo6 O7 94.1(3) . . ?
O25 Mo6 O10 98.2(3) . . ?
O25 Mo6 O20 103.3(3) . . ?
O25 Mo6 O23 108.2(3) . . ?
Mo6 Mo6' Mo2 129.4(4) . . ?
Mo6 Mo6' O6 90.8(4) . . ?
Mo6 Mo6' O7 133.3(4) . . ?
Mo6 Mo6' O10 118.0(4) . . ?
Mo6 Mo6' O20 45.7(3) . . ?
Mo6 Mo6' O23 38.6(3) . . ?
Mo6 Mo6' O25 65.3(4) . . ?
O6 Mo6' Mo2 50.86(14) . . ?
O7 Mo6' Mo2 32.1(2) . . ?
O7 Mo6' O6 81.7(3) . . ?
O7 Mo6' O10 108.4(3) . . ?
O7 Mo6' O20 89.2(3) . . ?
O7 Mo6' O23 159.4(3) . . ?
O7 Mo6' O25 106.8(3) . . ?
O10 Mo6' Mo2 98.2(2) . . ?
O10 Mo6' O6 93.0(2) . . ?
O10 Mo6' O20 154.1(3) . . ?
O10 Mo6' O23 81.6(3) . . ?
O10 Mo6' O25 106.9(3) . . ?
O20 Mo6' Mo2 86.62(16) . . ?
O20 Mo6' O6 70.4(2) . . ?
O20 Mo6' O23 76.2(2) . . ?
O23 Mo6' Mo2 130.64(18) . . ?
O23 Mo6' O6 79.8(2) . . ?
O25 Mo6' Mo2 138.2(3) . . ?
O25 Mo6' O6 154.0(3) . . ?
O25 Mo6' O20 85.0(3) . . ?
O25 Mo6' O23 86.5(3) . . ?
O3 Mo7 Mo4' 86.61(16) . . ?
O3 Mo7 O4 73.58(19) . . ?
O4 Mo7 Mo4' 48.73(13) . . ?
O5 Mo7 Mo4' 26.74(16) . . ?
O5 Mo7 O3 88.9(2) . . ?
O5 Mo7 O4 74.8(2) . . ?
O5 Mo7 O13 158.9(2) . . ?
O8 Mo7 Mo4' 86.64(17) . . ?
O8 Mo7 O3 159.8(2) . . ?
O8 Mo7 O4 87.7(2) . . ?
O8 Mo7 O5 93.5(2) . . ?
O8 Mo7 O13 85.0(2) . . ?
O13 Mo7 Mo4' 132.34(16) . . ?
O13 Mo7 O3 85.5(2) . . ?
O13 Mo7 O4 84.07(19) . . ?
O34 Mo7 Mo4' 127.3(2) . . ?
O34 Mo7 O3 97.1(2) . . ?
O34 Mo7 O4 169.5(2) . . ?
O34 Mo7 O5 100.5(3) . . ?
O34 Mo7 O8 102.1(2) . . ?
O34 Mo7 O13 100.4(3) . . ?
O10 Mo8 O16 86.85(19) . . ?
O10 Mo8 O19 93.1(2) . . ?
O10 Mo8 O29 158.0(2) . . ?
O10 Mo8 O31 85.2(2) . . ?
O15 Mo8 O10 103.7(2) . . ?
O15 Mo8 O16 169.2(2) . . ?
O15 Mo8 O19 102.2(3) . . ?
O15 Mo8 O29 97.4(2) . . ?
O15 Mo8 O31 99.7(3) . . ?
O19 Mo8 O16 74.4(2) . . ?
O19 Mo8 O29 88.1(2) . . ?
O19 Mo8 O31 157.8(2) . . ?
O29 Mo8 O16 72.33(19) . . ?
O31 Mo8 O16 83.4(2) . . ?
O31 Mo8 O29 85.5(2) . . ?
Mo9' Mo9 O8 55.6(4) . . ?
Mo9' Mo9 O16 91.7(4) . . ?
Mo9' Mo9 O17 140.9(4) . . ?
Mo9' Mo9 O29 117.6(4) . . ?
Mo9' Mo9 O38 33.7(4) . . ?
Mo9' Mo9 O40 75.5(4) . . ?
O8 Mo9 O16 82.89(18) . . ?
O8 Mo9 O38 80.3(2) . . ?
O17 Mo9 O8 85.8(2) . . ?
O17 Mo9 O16 89.4(2) . . ?
O17 Mo9 O29 100.5(3) . . ?
O17 Mo9 O38 157.1(2) . . ?
O29 Mo9 O8 157.5(2) . . ?
O29 Mo9 O16 75.7(2) . . ?
O29 Mo9 O38 86.4(2) . . ?
O38 Mo9 O16 71.05(19) . . ?
O40 Mo9 O8 96.2(3) . . ?
O40 Mo9 O16 164.7(3) . . ?
O40 Mo9 O17 105.8(3) . . ?
O40 Mo9 O29 102.7(3) . . ?
O40 Mo9 O38 93.8(3) . . ?
Mo9 Mo9' Mo10 115.0(4) . . ?
Mo9 Mo9' O8 108.5(5) . . ?
Mo9 Mo9' O16 73.8(4) . . ?
Mo9 Mo9' O17 29.5(3) . . ?
Mo9 Mo9' O29 48.2(4) . . ?
Mo9 Mo9' O38 134.7(5) . . ?
Mo9 Mo9' O40 84.4(5) . . ?
O8 Mo9' Mo10 93.3(2) . . ?
O8 Mo9' O16 86.2(2) . . ?
O8 Mo9' O17 79.5(3) . . ?
O8 Mo9' O29 148.3(3) . . ?
O16 Mo9' Mo10 46.85(14) . . ?
O17 Mo9' Mo10 123.28(18) . . ?
O17 Mo9' O16 76.5(2) . . ?
O29 Mo9' Mo10 82.34(17) . . ?
O29 Mo9' O16 68.0(2) . . ?
O29 Mo9' O17 77.0(2) . . ?
O38 Mo9' Mo10 30.05(18) . . ?
O38 Mo9' O8 102.7(3) . . ?
O38 Mo9' O16 76.5(2) . . ?
O38 Mo9' O17 152.6(3) . . ?
O38 Mo9' O29 89.1(3) . . ?
O38 Mo9' O40 115.5(4) . . ?
O40 Mo9' Mo10 144.5(3) . . ?
O40 Mo9' O8 109.0(3) . . ?
O40 Mo9' O16 156.6(3) . . ?
O40 Mo9' O17 88.6(3) . . ?
O40 Mo9' O29 91.4(3) . . ?
O16 Mo10 Mo9' 49.27(13) . . ?
O19 Mo10 Mo9' 85.59(17) . . ?
O19 Mo10 O16 73.3(2) . . ?
O22 Mo10 Mo9' 87.17(17) . . ?
O22 Mo10 O16 86.8(2) . . ?
O22 Mo10 O19 158.6(2) . . ?
O22 Mo10 O26 84.4(2) . . ?
O26 Mo10 Mo9' 132.87(17) . . ?
O26 Mo10 O16 83.95(19) . . ?
O26 Mo10 O19 85.9(2) . . ?
O33 Mo10 Mo9' 125.7(2) . . ?
O33 Mo10 O16 171.0(2) . . ?
O33 Mo10 O19 99.8(2) . . ?
O33 Mo10 O22 100.8(3) . . ?
O33 Mo10 O26 101.4(2) . . ?
O33 Mo10 O38 99.9(3) . . ?
O38 Mo10 Mo9' 25.80(18) . . ?
O38 Mo10 O16 74.7(2) . . ?
O38 Mo10 O19 89.0(2) . . ?
O38 Mo10 O22 93.2(2) . . ?
O38 Mo10 O26 158.6(2) . . ?
O3 Mo11 O4 74.83(19) . . ?
O3 Mo11 O11 158.2(2) . . ?
O3 Mo11 O27 88.3(2) . . ?
O9 Mo11 O3 92.9(2) . . ?
O9 Mo11 O4 86.8(2) . . ?
O9 Mo11 O11 85.1(2) . . ?
O9 Mo11 O27 158.5(2) . . ?
O11 Mo11 O4 83.42(19) . . ?
O27 Mo11 O4 72.74(19) . . ?
O27 Mo11 O11 86.0(2) . . ?
O39 Mo11 O3 102.4(2) . . ?
O39 Mo11 O4 169.7(2) . . ?
O39 Mo11 O9 103.3(3) . . ?
O39 Mo11 O11 99.2(2) . . ?
O39 Mo11 O27 97.4(2) . . ?
O6 Mo12 Mo2' 47.11(14) . . ?
O11 Mo12 Mo2' 82.81(16) . . ?
O11 Mo12 O6 86.68(19) . . ?
O11 Mo12 O12 92.9(2) . . ?
O11 Mo12 O18 86.0(2) . . ?
O11 Mo12 O20 159.2(2) . . ?
O12 Mo12 Mo2' 28.74(15) . . ?
O12 Mo12 O6 74.35(19) . . ?
O12 Mo12 O18 157.9(2) . . ?
O12 Mo12 O20 87.2(2) . . ?
O14 Mo12 Mo2' 131.0(2) . . ?
O14 Mo12 O6 169.2(2) . . ?
O14 Mo12 O11 103.9(2) . . ?
O14 Mo12 O12 102.4(2) . . ?
O14 Mo12 O18 99.2(2) . . ?
O14 Mo12 O20 96.3(2) . . ?
O18 Mo12 Mo2' 129.80(16) . . ?
O18 Mo12 O6 83.6(2) . . ?
O18 Mo12 O20 86.1(2) . . ?
O20 Mo12 Mo2' 87.55(17) . . ?
O20 Mo12 O6 73.36(19) . . ?
N1 Cu1 N2 176.1(3) . . ?
N1 Cu1 O43 97.3(3) . . ?
N2 Cu1 O43 82.7(2) . . ?
O42 Cu1 N1 83.4(3) . . ?
O42 Cu1 N2 96.5(2) . . ?
O42 Cu1 O43 178.2(3) . . ?
N3 Cu2 N3 180.00(14) . 3_666 ?
N3 Cu2 O3W 87.1(3) 3_666 . ?
N3 Cu2 O3W 92.9(3) 3_666 3_666 ?
N3 Cu2 O3W 87.1(3) . 3_666 ?
N3 Cu2 O3W 92.9(3) . . ?
N3 Cu2 O45 97.3(2) 3_666 . ?
N3 Cu2 O45 82.7(2) . . ?
N3 Cu2 O45 82.7(2) 3_666 3_666 ?
N3 Cu2 O45 97.3(2) . 3_666 ?
O3W Cu2 O3W 180.0 . 3_666 ?
O45 Cu2 O3W 88.2(3) 3_666 . ?
O45 Cu2 O3W 91.8(3) 3_666 3_666 ?
O45 Cu2 O3W 91.8(3) . . ?
O45 Cu2 O3W 88.2(3) . 3_666 ?
O45 Cu2 O45 180.0 . 3_666 ?
N4 Cu3 N5 179.5(4) . . ?
N4 Cu3 O49 98.7(3) . . ?
N5 Cu3 O49 81.9(3) . . ?
O48 Cu3 N4 86.6(4) . . ?
O48 Cu3 N5 92.9(3) . . ?
O48 Cu3 O49 174.7(3) . . ?
C1 N1 Cu1 128.9(6) . . ?
C5 N1 Cu1 111.7(5) . . ?
C5 N1 C1 119.1(7) . . ?
C7 N2 Cu1 128.7(6) . . ?
C7 N2 C11 118.8(7) . . ?
C11 N2 Cu1 112.5(5) . . ?
C13 N3 Cu2 128.4(6) . . ?
C17 N3 Cu2 112.8(5) . . ?
C17 N3 C13 118.8(7) . . ?
C19 N4 Cu3 129.1(8) . . ?
C23 N4 Cu3 111.1(7) . . ?
C23 N4 C19 119.8(9) . . ?
C25 N5 Cu3 127.3(6) . . ?
C25 N5 C29 118.8(8) . . ?
C29 N5 Cu3 113.8(6) . . ?
Ce1' O5W Ce1 19.80(9) . . ?
Ce1' O7W Ce1 19.73(10) . . ?
Ce1' O8W Ce1 7.50(14) . . ?
Mo1 O1 Mo1' 23.18(12) . . ?
Ge1 O2 Mo1 123.0(3) . . ?
Ge1 O2 Mo1' 120.0(3) . . ?
Ge1 O2 Mo3 122.4(3) . . ?
Ge1 O2 Mo3' 124.1(3) . . ?
Ge1 O2 Mo5 122.0(3) . . ?
Mo1 O2 Mo1' 16.88(7) . . ?
Mo1 O2 Mo3 92.58(19) . . ?
Mo1 O2 Mo5 96.59(19) . . ?
Mo3 O2 Mo1' 105.9(2) . . ?
Mo3' O2 Mo1 80.7(2) . . ?
Mo3' O2 Mo1' 95.4(2) . . ?
Mo3' O2 Mo3 13.83(8) . . ?
Mo3' O2 Mo5 100.7(2) . . ?
Mo5 O2 Mo1' 85.73(18) . . ?
Mo5 O2 Mo3 92.33(19) . . ?
Mo11 O3 Mo7 118.2(2) . . ?
Ge1 O4 Mo4 121.9(2) . . ?
Ge1 O4 Mo4' 124.5(3) . . ?
Ge1 O4 Mo7 122.4(3) . . ?
Ge1 O4 Mo11 122.4(3) . . ?
Mo4 O4 Mo4' 15.91(7) . . ?
Mo4 O4 Mo11 91.56(18) . . ?
Mo7 O4 Mo4 97.43(18) . . ?
Mo7 O4 Mo4' 83.85(17) . . ?
Mo7 O4 Mo11 93.39(17) . . ?
Mo11 O4 Mo4' 100.6(2) . . ?
Mo4' O5 Mo4 12.38(12) . . ?
Mo4' O5 Mo7 121.5(3) . . ?
Mo7 O5 Mo4 116.9(2) . . ?
Ge1 O6 Mo2 123.1(3) . . ?
Ge1 O6 Mo2' 118.6(3) . . ?
Ge1 O6 Mo6 122.4(2) . . ?
Ge1 O6 Mo6' 122.9(3) . . ?
Ge1 O6 Mo12 123.1(3) . . ?
Mo2 O6 Mo2' 14.71(7) . . ?
Mo2 O6 Mo6 92.61(17) . . ?
Mo6 O6 Mo2' 105.4(2) . . ?
Mo6' O6 Mo2 80.02(18) . . ?
Mo6' O6 Mo2' 93.9(2) . . ?
Mo6' O6 Mo6 15.52(8) . . ?
Mo6' O6 Mo12 101.7(2) . . ?
Mo12 O6 Mo2 95.74(18) . . ?
Mo12 O6 Mo2' 88.14(18) . . ?
Mo12 O6 Mo6 91.57(17) . . ?
Mo2 O7 Mo2' 8.00(9) . . ?
Mo2 O7 Mo6 120.0(3) . . ?
Mo6 O7 Mo2' 116.4(2) . . ?
Mo6' O7 Mo2 119.0(3) . . ?
Mo6' O7 Mo2' 117.3(3) . . ?
Mo6' O7 Mo6 12.57(12) . . ?
Mo7 O8 Mo9 148.4(3) . . ?
Mo9' O8 Mo7 162.5(3) . . ?
Mo9' O8 Mo9 15.92(11) . . ?
Mo3' O9 Mo3 14.57(11) . . ?
Mo3' O9 Mo11 158.3(3) . . ?
Mo11 O9 Mo3 151.0(3) . . ?
Mo6' O10 Mo6 15.34(12) . . ?
Mo6' O10 Mo8 160.1(3) . . ?
Mo8 O10 Mo6 150.6(3) . . ?
Mo12 O11 Mo11 151.8(3) . . ?
Mo2' O12 Mo2 16.44(10) . . ?
Mo2' O12 Mo12 121.4(3) . . ?
Mo12 O12 Mo2 119.2(2) . . ?
Mo1 O13 Mo1' 16.06(9) . . ?
Mo1 O13 Mo7 156.6(3) . . ?
Mo7 O13 Mo1' 142.7(3) . . ?
Ce1' O14 Ce1 18.98(8) . . ?
Mo12 O14 Ce1 168.6(3) . . ?
Mo12 O14 Ce1' 149.6(3) . . ?
Ge1 O16 Mo8 123.0(3) . . ?
Ge1 O16 Mo9 122.0(3) . . ?
Ge1 O16 Mo9' 125.0(3) . . ?
Ge1 O16 Mo10 122.6(3) . . ?
Mo8 O16 Mo9' 99.1(2) . . ?
Mo9 O16 Mo8 91.50(17) . . ?
Mo9 O16 Mo9' 14.53(8) . . ?
Mo9 O16 Mo10 96.64(19) . . ?
Mo10 O16 Mo8 93.21(18) . . ?
Mo10 O16 Mo9' 83.88(19) . . ?
Mo1 O17 Mo9' 144.3(3) . . ?
Mo1' O17 Mo1 14.25(13) . . ?
Mo1' O17 Mo9 165.4(4) . . ?
Mo1' O17 Mo9' 158.3(4) . . ?
Mo9 O17 Mo1 152.4(3) . . ?
Mo9 O17 Mo9' 9.62(11) . . ?
Mo3 O18 Mo3' 11.27(10) . . ?
Mo3 O18 Mo12 156.0(3) . . ?
Mo12 O18 Mo3' 144.8(3) . . ?
Mo8 O19 Mo10 119.1(3) . . ?
Mo6 O20 Mo6' 14.26(10) . . ?
Mo6 O20 Mo12 120.0(3) . . ?
Mo12 O20 Mo6' 113.1(2) . . ?
Mo2 O21 Mo4' 142.7(3) . . ?
Mo2' O21 Mo2 9.80(12) . . ?
Mo2' O21 Mo4 161.8(4) . . ?
Mo2' O21 Mo4' 152.4(3) . . ?
Mo4 O21 Mo2 152.5(3) . . ?
Mo4 O21 Mo4' 10.77(9) . . ?
Mo4' O22 Mo4 17.01(10) . . ?
Mo4' O22 Mo10 163.6(3) . . ?
Mo10 O22 Mo4 149.0(3) . . ?
Mo5 O23 Mo6' 143.2(3) . . ?
Mo6 O23 Mo5 155.6(3) . . ?
Mo6 O23 Mo6' 12.61(9) . . ?
Mo4 O24 Mo4' 21.49(11) . . ?
Mo6 O25 Mo6' 19.90(11) . . ?
Mo2 O26 Mo2' 15.75(9) . . ?
Mo2 O26 Mo10 156.9(3) . . ?
Mo10 O26 Mo2' 143.4(3) . . ?
Mo4 O27 Mo4' 14.82(9) . . ?
Mo4 O27 Mo11 119.7(3) . . ?
Mo11 O27 Mo4' 117.0(3) . . ?
Mo1 O28 Mo1' 11.02(10) . . ?
Mo1 O28 Mo3 120.3(3) . . ?
Mo3 O28 Mo1' 116.6(3) . . ?
Mo3' O28 Mo1 117.3(4) . . ?
Mo3' O28 Mo1' 115.7(3) . . ?
Mo3' O28 Mo3 10.13(14) . . ?
Mo8 O29 Mo9' 119.1(3) . . ?
Mo9 O29 Mo8 120.1(3) . . ?
Mo9 O29 Mo9' 14.20(11) . . ?
Mo5 O31 Mo8 152.1(3) . . ?
Mo1' O32 Mo1 18.14(11) . . ?
Mo1' O32 Mo5 121.7(3) . . ?
Mo5 O32 Mo1 118.2(3) . . ?
Mo2 O35 Mo2' 20.03(11) . . ?
Mo3 O36 Mo3' 17.19(12) . . ?
Mo3 O37 Mo3' 14.09(10) . . ?
Mo3 O37 Mo5 120.8(3) . . ?
Mo5 O37 Mo3' 112.9(3) . . ?
Mo9' O38 Mo9 11.63(13) . . ?
Mo9' O38 Mo10 124.1(3) . . ?
Mo10 O38 Mo9 117.6(3) . . ?
Mo9' O40 Mo9 20.19(12) . . ?
C6 O42 Cu1 114.4(5) . . ?
C12 O43 Cu1 114.0(5) . . ?
Ce1' O44 Ce1 20.21(9) . . ?
C12 O44 Ce1 142.7(6) . . ?
C12 O44 Ce1' 145.2(6) . . ?
C18 O45 Cu2 114.2(5) . . ?
Ce1 O46 Ce1' 19.00(8) . . ?
C18 O46 Ce1 143.4(5) . . ?
C18 O46 Ce1' 145.0(5) . . ?
C24 O48 Cu3 111.5(7) . . ?
C30 O49 Cu3 114.2(6) . . ?
C30 O50 Ce1 148.6(6) . . ?
N1 C1 C2 121.6(8) . . ?
C1 C2 C3 119.4(8) . . ?
C4 C3 C2 118.7(7) . . ?
C3 C4 C5 119.6(7) . . ?
N1 C5 C4 121.6(7) . . ?
N1 C5 C6 115.7(7) . . ?
C4 C5 C6 122.7(7) . . ?
O41 C6 O42 123.2(8) . . ?
O41 C6 C5 122.3(8) . . ?
O42 C6 C5 114.5(7) . . ?
N2 C7 C8 122.5(8) . . ?
C7 C8 C9 118.4(8) . . ?
C10 C9 C8 118.7(8) . . ?
C9 C10 C11 119.6(8) . . ?
N2 C11 C10 122.0(8) . . ?
N2 C11 C12 114.4(7) . . ?
C10 C11 C12 123.5(7) . . ?
O43 C12 C11 115.8(7) . . ?
O44 C12 O43 124.8(8) . . ?
O44 C12 C11 119.4(7) . . ?
N3 C13 C14 121.6(8) . . ?
C15 C14 C13 119.7(8) . . ?
C14 C15 C16 118.9(8) . . ?
C15 C16 C17 118.5(8) . . ?
N3 C17 C16 122.4(7) . . ?
N3 C17 C18 114.8(7) . . ?
C16 C17 C18 122.8(8) . . ?
O45 C18 C17 115.4(7) . . ?
O46 C18 O45 125.7(7) . . ?
O46 C18 C17 118.9(7) . . ?
N4 C19 C20 119.8(12) . . ?
C21 C20 C19 119.3(11) . . ?
C22 C21 C20 120.8(10) . . ?
C21 C22 C23 117.1(12) . . ?
N4 C23 C22 123.1(11) . . ?
N4 C23 C24 115.0(9) . . ?
C22 C23 C24 121.9(11) . . ?
O47 C24 O48 121.4(12) . . ?
O47 C24 C23 122.9(11) . . ?
O48 C24 C23 115.7(10) . . ?
N5 C25 C26 121.7(9) . . ?
C25 C26 C27 119.0(10) . . ?
C28 C27 C26 119.2(10) . . ?
C27 C28 C29 119.8(10) . . ?
N5 C29 C28 121.4(9) . . ?
N5 C29 C30 113.4(8) . . ?
C28 C29 C30 125.2(9) . . ?
O49 C30 C29 116.8(8) . . ?
O50 C30 O49 123.2(9) . . ?
O50 C30 C29 120.0(9) . . ?

_smtbx_masks_special_details     ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 -0.037 -0.082 0.369 10.8 0.8 ?
2 0.037 0.082 0.631 10.8 0.9 ?
3 0.037 0.418 0.131 10.8 0.9 ?
4 -0.037 0.582 0.869 10.8 0.8 ?
5 0.118 0.056 0.467 18.6 8.8 ?
6 0.118 0.444 0.967 18.6 8.7 ?
7 0.500 0.000 0.500 315.7 84.9 ?
8 0.500 0.500 1.000 315.7 84.9 ?
9 0.882 0.556 0.033 18.6 8.3 ?
10 0.882 0.944 0.533 18.6 8.2 ?

_olex2_exptl_crystal_mounting_method ?
_olex2_submission_special_instructions 'No special instructions were received'
